Home >
Documents >
Theelectronicproperties of bilayer graphene · graphene [40], twisted graphene [41–46] or two...

Share this document with a friend

Embed Size (px)

of 31
/31

Transcript

The electronic properties of bilayer graphene

Edward McCannDepartment of Physics, Lancaster University, Lancaster, LA1 4YB, UK

Mikito KoshinoDepartment of Physics, Tohoku University, Sendai, 980-8578, Japan

We review the electronic properties of bilayer graphene, beginning with a description of the tight-binding model of bilayer graphene and the derivation of the effective Hamiltonian describing massivechiral quasiparticles in two parabolic bands at low energy. We take into account five tight-bindingparameters of the Slonczewski-Weiss-McClure model of bulk graphite plus intra- and interlayerasymmetry between atomic sites which induce band gaps in the low-energy spectrum. The Hartreemodel of screening and band-gap opening due to interlayer asymmetry in the presence of externalgates is presented. The tight-binding model is used to describe optical and transport propertiesincluding the integer quantum Hall effect, and we also discuss orbital magnetism, phonons and theinfluence of strain on electronic properties. We conclude with an overview of electronic interactioneffects.

CONTENTS

I. Introduction 1

II. Electronic band structure 2A. The crystal structure and the Brillouin

zone 2B. The tight-binding model 3

1. An arbitrary crystal structure 32. Monolayer graphene 43. Bilayer graphene 54. Effective four-band Hamiltonian near theK points 7

C. Effective two-band Hamiltonian at lowenergy 71. General procedure 72. Bilayer graphene 8

D. Interlayer coupling γ1: massive chiralelectrons 8

E. Interlayer coupling γ3: trigonal warping andthe Lifshitz transition 9

F. Interlayer coupling γ4 and on-site parameter∆′: electron-hole asymmetry 9

G. Asymmetry between on-site energies: bandgaps 91. Interlayer asymmetry 92. Intralayer asymmetry between A and B

sites 10H. Next-nearest neighbour hopping 10I. Spin-orbit coupling 10J. The integer quantum Hall effect 11

1. The Landau level spectrum of bilayergraphene 11

2. Three types of integer quantum Halleffect 12

3. The role of interlayer asymmetry 13

III. Tuneable band gap 13A. Experiments 13B. Hartree model of screening 13

1. Electrostatics: asymmetry parameter,layer densities and external gates 13

2. Calculation of individual layer densities 143. Self-consistent screening 15

IV. Transport properties 16A. Introduction 16B. Ballistic transport in a finite system 16C. Transport in disordered bilayer graphene 18

1. Conductivity 182. Localisation effects 20

V. Optical properties 20

VI. Orbital magnetism 21

VII. Phonons and strain 22A. The influence of strain on electrons in

bilayer graphene 22B. Phonons in bilayer graphene 22C. Optical phonon anomaly 23

VIII. Electronic interactions 24

IX. Summary 25

References 26

I. INTRODUCTION

The production by mechanical exfoliation of isolatedflakes of graphene with excellent conducting properties[1] was soon followed by the observation of an unusualsequence of plateaus in the integer quantum Hall effect inmonolayer graphene [2, 3]. This confirmed the fact thatcharge carriers in monolayer graphene are massless chiralquasiparticles with a linear dispersion, as described by aDirac-like effective Hamiltonian [4–6], and it promptedan explosion of interest in the field [7].

2

The integer quantum Hall effect in bilayer graphene [8]is arguably even more unusual than in monolayer becauseit indicates the presence of massive chiral quasiparticles[9] with a parabolic dispersion at low energy. The effec-tive Hamiltonian of bilayer graphene may be viewed asa generalisation of the Dirac-like Hamiltonian of mono-layer graphene and the second (after the monolayer) in afamily of chiral Hamiltonians that appear at low energyin ABC-stacked (rhombohedral) multilayer graphene [9–15]. In addition to interesting underlying physics, bilayergraphene holds potential for electronics applications, notleast because of the possibility to control both carrierdensity and energy band gap through doping or gating[9, 10, 16–20].

Not surprisingly, many of the properties of bilayergraphene are similar to those in monolayer [7, 21]. Theseinclude excellent electrical conductivity with room tem-perature mobility of up to 40, 000 cm2V−1 s−1 in air [22];the possibility to tune electrical properties by changingthe carrier density through gating or doping [1, 8, 16];high thermal conductivity with room temperature ther-mal conductivity of about 2, 800Wm−1K−1 [23, 24]; me-chanical stiffness, strength and flexibility (Young’s mod-ulus is estimated to be about 0.8TPa [25, 26]); trans-parency with transmittance of white light of about 95%[27]; impermeability to gases [28]; and the ability to bechemically functionalised [29]. Thus, as with monolayergraphene, bilayer graphene has potential for future appli-cations in many areas [21] including transparent, flexibleelectrodes for touch screen displays [30]; high-frequencytransistors [31]; thermoelectric devices [32]; photonic de-vices including plasmonic devices [33] and photodetectors[34]; energy applications including batteries [35, 36]; andcomposite materials [37, 38].

It should be stressed, however, that bilayer graphenehas features that make it distinct from monolayer. Thelow-energy band structure, described in detail in Sec-tion II, is different. Like monolayer, intrinsic bilayer hasno band gap between its conduction and valence bands,but the low-energy dispersion is quadratic (rather thanlinear as in monolayer) with massive chiral quasiparti-cles [8, 9] rather than massless ones. As there are twolayers, bilayer graphene represents the thinnest possiblelimit of an intercalated material [35, 36]. It is possibleto address each layer separately leading to entirely newfunctionalities in bilayer graphene including the possibil-ity to control an energy band gap of up to about 300meVthrough doping or gating [9, 10, 16–20]. Recently, thisband gap has been used to create devices - constrictionsand dots - by electrostatic confinement with gates [39].Bilayer or multilayer graphene devices may also be prefer-able to monolayer ones when there is a need to use morematerial for increased electrical or thermal conduction,strength [37, 38], or optical signature [33].

In the following we review the electronic propertiesof bilayer graphene. Section II is an overview of theelectronic tight-binding Hamiltonian and resulting bandstructure describing the low-energy chiral Hamiltonian

and taking into account different parameters that cou-ple atomic orbitals as well as external factors that maychange the electron bands by, for example, opening aband gap. We include the Landau level spectrum in thepresence of a perpendicular magnetic field and the corre-sponding integer quantum Hall effect. In section III weconsider the opening of a band gap due to doping or gat-ing and present a simple analytical model that describesthe density-dependence of the band gap by taking intoaccount screening by electrons on the bilayer device. Thetight-binding model is used to describe transport prop-erties, section IV, and optical properties, section V. Wealso discuss orbital magnetism in section VI, phononsand the influence of strain in section VII. Section VIIIconcludes with an overview of electronic-interaction ef-fects. Note that this review considers Bernal-stacked(also known as AB-stacked) bilayer graphene; we donot consider other stacking types such as AA-stackedgraphene [40], twisted graphene [41–46] or two graphenesheets separated by a dielectric with, possibly, electronicinteractions between them [47–52].

II. ELECTRONIC BAND STRUCTURE

A. The crystal structure and the Brillouin zone

Bilayer graphene consists of two coupled monolayersof carbon atoms, each with a honeycomb crystal struc-ture. Figure 1 shows the crystal structure of monolayergraphene, figure 2 shows bilayer graphene. In both cases,primitive lattice vectors a1 and a2 may be defined as

a1 =

(

a

2,

√3a

2

)

, a2 =

(

a

2,−

√3a

2

)

, (1)

where a = |a1| = |a2| is the lattice constant, the distancebetween adjacent unit cells, a = 2.46 A [53]. Note thatthe lattice constant is distinct from the carbon-carbonbond length aCC = a/

√3 = 1.42 A, which is the distance

between adjacent carbon atoms.In monolayer graphene, each unit cell contains two

carbon atoms, labelled A and B, figure 1(a). The po-sitions of A and B atoms are not equivalent because itis not possible to connect them with a lattice vector ofthe form R = n1a1 + n2a2, where n1 and n2 are inte-gers. Bilayer graphene consists of two coupled monolay-ers, with four atoms in the unit cell, labelled A1, B1on the lower layer and A2, B2 on the upper layer. Thelayers are arranged so that one of the atoms from thelower layer B1 is directly below an atom, A2, from theupper layer. We refer to these two atomic sites as ‘dimer’sites because the electronic orbitals on them are cou-pled together by a relatively strong interlayer coupling.The other two atoms, A1 and B2, don’t have a counter-part on the other layer that is directly above or belowthem, and are referred to as ‘non-dimer’ sites. Note thatsome authors [10, 54–56] employ different definitions of

3

B

A

x

ya

a1

a2

b1

b2

k y

k x K +K -

M

G

( a )

( b )

FIG. 1. (a) Crystal structure of monolayer graphene withA (B) atoms shown as white (black) circles. The shadedrhombus is the conventional unit cell, a1 and a2 are primitivelattice vectors. (b) Reciprocal lattice of monolayer and bilayergraphene with lattice points indicated as crosses, b1 and b2

are primitive reciprocal lattice vectors. The shaded hexagonis the first Brillouin zone with Γ indicating the centre, andK+ and K− showing two non-equivalent corners.

A and B sites as used here. The point group of the bi-layer crystal structure is D3d [12, 57, 58] consisting ofelements (E, 2C3, 3C

′2, i, 2S6, 3σd), and it may be re-

garded as a direct product of group D3 (E, 2C3, 3C′2)

with the inversion group Ci (E, i). Thus, the latticeis symmetric with respect to spatial inversion symmetry(x, y, z) → (−x,−y,−z).Primitive reciprocal lattice vectors b1 and b2 of mono-

layer and bilayer graphene, where a1 · b1 = a2 · b2 = 2πand a1 · b2 = a2 · b1 = 0, are given by

b1 =

(

2π

a,2π√3a

)

, b2 =

(

2π

a,− 2π√

3a

)

. (2)

As shown in figure 1(b), the reciprocal lattice is an hexag-onal Bravais lattice, and the first Brillouin zone is anhexagon.

B 2A 1

x

ya

a1

a2

( a )

A 2

B 1

A 1

B 2

B 1

A 2

g 1

g 1

g 0

g 0

( b )

g 3

ag 4

FIG. 2. (a) Plan and (b) side view of the crystal structure ofbilayer graphene. Atoms A1 and B1 on the lower layer areshown as white and black circles, A2, B2 on the upper layerare black and grey, respectively. The shaded rhombus in (a)indicates the conventional unit cell.

B. The tight-binding model

1. An arbitrary crystal structure

In the following, we will describe the tight-bindingmodel [53, 59, 60] and its application to bilayer graphene.We begin by considering an arbitrary crystal with trans-lational invariance and M atomic orbitals φm per unitcell, labelled by index m = 1 . . .M . Bloch statesΦm(k, r) for a given position vector r and wave vectork may be written as

Φm(k, r) =1√N

N∑

i=1

eik.Rm,iφm (r−Rm,i) , (3)

where N is the number of unit cells, i = 1 . . .N labelsthe unit cell, and Rm,i is the position vector of the mthorbital in the ith unit cell.The electronic wave function Ψj(k, r) may be ex-

pressed as a linear superposition of Bloch states

Ψj(k, r) =

M∑

m=1

ψj,m(k)Φm(k, r) , (4)

where ψj,m are expansion coefficients. There are M dif-ferent energy bands, and the energy Ej(k) of the jthband is given by Ej(k) = 〈Ψj |H|Ψj〉/〈Ψj |Ψj〉 where His the Hamiltonian. Minimising the energy Ej with re-spect to the expansion coefficients ψj,m [53, 60] leads to

Hψj = EjSψj , (5)

4

where ψj is a column vector, ψTj = (ψj1, ψj2, . . . , ψjM ).

The transfer integral matrix H and overlap integral ma-trix S areM ×M matrices with matrix elements definedby

Hmm′ = 〈Φm|H|Φm′〉 , Smm′ = 〈Φm|Φm′〉 . (6)

The band energies Ej may be determined from the gen-eralised eigenvalue equation (5) by solving the secularequation

det (H − EjS) = 0 , (7)

where ‘det’ stands for the determinant of the matrix.In order to model a given system in terms of the gener-

alised eigenvalue problem (5), it is necessary to determinethe matrices H and S. We will proceed by consideringthe relatively simple case of monolayer graphene, beforegeneralising the approach to bilayers. In the followingsections, we will omit the subscript j on ψj and Ej inequation (5), remembering that the number of solutionsis M , the number of orbitals per unit cell.

2. Monolayer graphene

Here, we will outline how to apply the tight-bindingmodel to graphene, and refer the reader to tutorial-stylereviews [53, 60] for further details. We take into accountone 2pz orbital per atomic site and, as there are twoatoms in the unit cell of monolayer graphene, figure 1(a),we include two orbitals per unit cell labelled as m = Aand m = B (the A atoms and the B atoms are eacharranged on an hexagonal Bravais lattice).We begin by considering the diagonal element HAA

of the transfer integral matrix H , equation (6), for theA site orbital. It may be determined by substituting theBloch function (3) form = A into the matrix element (6),which results in a double sum over the positions of theunit cells in the crystal. Assuming that the dominantcontribution arises from those terms involving a givenorbital interacting with itself (i.e., in the same unit cell),the matrix element may be written as

HAA ≈ 1

N

N∑

i=1

〈φA (r−RA,i) |H|φA (r−RA,i)〉 . (8)

This may be regarded as a summation over all unit cells ofa parameter ǫA = 〈φA (r−RA,i) |H|φA (r−RA,i)〉 thattakes the same value in every unit cell. Thus, the matrixelement may be simply expressed as HAA ≈ ǫA. Simi-larly, the diagonal element HBB for the B site orbital canbe written as HBB = ǫB, while for intrinsic graphene ǫAis equal to ǫB as the two sublattices are identical. Thecalculation of the diagonal elements of the overlap inte-gral matrix S, equation (6), proceeds in the same wayas that of H , with the overlap of an orbital with itselfequal to unity, 〈φj (r−Rj,i) |φj (r−Rj,i)〉 = 1. Thus,SBB = SAA = 1.

The off-diagonal element HAB of the transfer integralmatrix H describes the possibility of hopping betweenorbitals on A and B sites. Substituting the Bloch func-tion (3) into the matrix element (6) results in a sum overall A sites and a sum over all B sites. We assume thatthe dominant contribution arises from hopping betweenadjacent sites. If we consider a given A site, say, then wetake into account the possibility of hopping to its threenearest-neighbour B sites, labelled by index l = 1, 2, 3:

HAB ≈ 1

N

N∑

i=1

3∑

l=1

eik.δl 〈φA (r−RA,i) |H|φB (r−RA,i − δl)〉 ,(9)

where δl are the positions of three nearest B atoms rel-ative to a given A atom, which may be written as δ1 =(

0, a/√3)

, δ2 =(

a/2,−a/2√3)

, δ3 =(

−a/2,−a/2√3)

.The sum with respect to the three nearest-neighbour

B sites is identical for every A site. A hopping parametermay be defined as

γ0 = −〈φA (r−RA,i) |H|φB (r−RA,i − δl)〉, (10)

which is positive. Then, the matrix element may be writ-ten as

HAB ≈ −γ0f (k) ; f (k) =

3∑

l=1

eik.δl , (11)

The other off-diagonal matrix element is given by HBA =H∗

AB ≈ −γ0f∗ (k). The function f (k) describingnearest-neighbor hopping, equation (11), is given by

f (k) = eikya/√3 + 2e−ikya/2

√3 cos (kxa/2) , (12)

where k = (kx, ky) is the in-plane wave vector. The cal-culation of the off-diagonal elements of the overlap in-tegral matrix S is similar to those of H . A parameters0 = 〈φA (r−RA,i) |φB (r−RB,l)〉 is introduced to de-scribe the possibility of non-zero overlap between orbitalson adjacent sites, giving SAB = S∗

BA = s0f (k).Gathering the matrix elements, the transfer Hm and

overlap Sm integral matrices of monolayer graphene maybe written as

Hm =

(

ǫA −γ0f (k)−γ0f∗ (k) ǫB

)

, (13)

Sm =

(

1 s0f (k)s0f

∗ (k) 1

)

. (14)

The corresponding energy may be determined [53] bysolving the secular equation (7). For intrinsic graphene,i.e., ǫA = ǫB = 0, we have

E± =±γ0|f (k) |1∓ s0|f (k) |

. (15)

The parameter values are listed by Saito et al [53] asγ0 = 3.033 eV and s0 = 0.129.The function f(k), equation (12) is zero at the corners

of the Brillouin zone, two of which are non-equivalent

5

(i.e., they are not connected by a reciprocal lattice vec-tor). For example, cornersK+ andK− with wave vectorsK± = ±(4π/3a, 0) are labelled in Figure 1(b). Such po-sitions are called K points or valleys, and we will use avalley index ξ = ±1 to distinguish points Kξ. At thesepositions, the solutions (15) are degenerate, marking acrossing point and zero band gap between the conductionand valence bands. The transfer matrix Hm is approxi-mately equal to a Dirac-like Hamiltonian in the vicinityof the K point, describing massless chiral quasiparticleswith a linear dispersion relation. These points are partic-ularly important because the Fermi level is located nearthem in pristine graphene.

3. Bilayer graphene

In the tight-binding description of bilayer graphene, wetake into account 2pz orbitals on the four atomic sites inthe unit cell, labelled as j = A1, B1, A2, B2. Then, thetransfer integral matrix of bilayer graphene [9, 10, 54, 61–63] is a 4× 4 matrix given by

Hb =

ǫA1 −γ0f (k) γ4f (k) −γ3f∗ (k)−γ0f∗ (k) ǫB1 γ1 γ4f (k)γ4f

∗ (k) γ1 ǫA2 −γ0f (k)−γ3f (k) γ4f

∗ (k) −γ0f∗ (k) ǫB2

,

(16)

where the tight-binding parameters are defined as

γ0 = −〈φA1|H|φB1〉 = −〈φA2|H|φB2〉, (17)

γ1 = 〈φA2|H|φB1〉, (18)

γ3 = −〈φA1|H|φB2〉, (19)

γ4 = 〈φA1|H|φA2〉 = 〈φB1|H|φB2〉. (20)

Here, we use the notation of the Slonczewski-Weiss-McClure (SWM) model [64–67] that describes bulkgraphite. Note that definitions of the parameters usedby authors can differ, particularly with respect to signs.The upper-left and lower-right square 2×2 blocks ofHb

describe intra-layer terms and are simple generalisationsof the monolayer, equation (13). For bilayer graphene,however, we include parameters describing the on-siteenergies ǫA1, ǫB1, ǫA2, ǫB2 on the four atomic sites, thatare not equal in the most general case. As there are foursites, differences between them are described by threeparameters [63]:

ǫA1 = 12 (−U + δAB) , (21)

ǫB1 = 12 (−U + 2∆′ − δAB) , (22)

ǫA2 = 12 (U + 2∆′ + δAB) , (23)

ǫB2 = 12 (U − δAB) . (24)

where

U = 12 [(ǫA1 + ǫB1)− (ǫA2 + ǫB2)] , (25)

∆′ = 12 [(ǫB1 + ǫA2)− (ǫA1 + ǫB2)] , (26)

δAB = 12 [(ǫA1 + ǫA2)− (ǫB1 + ǫB2)] . (27)

The three independent parameters are U to describe in-terlayer asymmetry between the two layers [9, 10, 16–20, 68–74], ∆′ for an energy difference between dimerand non-dimer sites [54–56, 67], and δAB for an energydifference between A and B sites on each layer [63, 75].These parameters are described in detail in sections II Fand IIG.The upper-right and lower-left square 2 × 2 blocks of

Hb describe inter-layer coupling. Parameter γ1 describescoupling between pairs of orbitals on the dimer sites B1and A2: since this is a vertical coupling, the correspond-ing terms in Hb (i.e., HA2,B1 = HB1,A2 = γ1) do notcontain f (k) which describes in-plane hopping. Param-eter γ3 describes interlayer coupling between non-dimerorbitals A1 and B2, and γ4 describes interlayer couplingbetween dimer and non-dimer orbitals A1 and A2 or B1and B2. Both γ3 and γ4 couplings are ‘skew’: they arenot strictly vertical, but involve a component of in-planehopping, and each atom on one layer (e.g., A1 for γ3) hasthree equidistant nearest-neighbours (e.g., B2 for γ3) onthe other layer. In fact, the in-plane component of thisskew hopping is analogous to nearest-neighbour hoppingwithin a single layer, as parameterised by γ0. Hence,the skew interlayer hopping (e.g., HA1,B2 = −γ3f∗ (k))contains the factor f (k) describing in-plane hopping.It is possible to introduce an overlap integral matrix

for bilayer graphene [63]

Sb =

1 s0f (k) 0 0

s0f∗ (k) 1 s1 0

0 s1 1 s0f (k)

0 0 s0f∗ (k) 1

, (28)

with a form that mirrors Hb. Here, we only includetwo parameters: s0 = 〈φA1|φB1〉 = 〈φA2|φB2〉 describingnon-orthogonality of intra-layer nearest-neighbours ands1 = 〈φA2|φB1〉 describing non-orthogonality of orbitalson dimer sites A1 and B2. In principle, it is possibleto introduce additional parameters analogous to γ3, γ4,etc., but generally they will be small and irrelevant. Infact, it is common practice to neglect the overlap inte-gral matrix entirely, i.e., replace Sb with a unit matrix,because the influence of parameters s0 and s1 describ-ing non-orthogonality of adjacent orbitals is small at lowenergy |E| ≤ γ1. Then, the generalised eigenvalue equa-tion (5) reduces to an eigenvalue equation Hbψ = Eψwith Hamiltonian Hb, equation (16).The energy differences U and δAB are usually at-

tributed to extrinsic factors such as gates, substratesor doping. Thus, there are five independent parame-ters in the Hamiltonian (16) of intrinsic bilayer graphene,namely γ0, γ1, γ3, γ4 and ∆′. The band structure pre-dicted by the tight-binding model has been compared toobservations from photoemission [16], Raman [76] andinfrared spectroscopy [55, 56, 78–81]. Parameter valuesdetermined by fitting to experiments are listed in Table Ifor bulk graphite [67], for bilayer graphene by Raman[76, 77] and infrared [55, 56, 80] spectroscopy, and for

6

TABLE I. Values (in eV) of the Slonczewski-Weiss-McClure (SWM) model parameters [64–67] determined experimentally.Numbers in parenthesis indicate estimated accuracy of the final digit(s). The energy difference between dimer and non-dimersites in the bilayer is ∆′ = ∆− γ2 + γ5. Note that next-nearest layer parameters γ2 and γ5 are not present in bilayer graphene.

Parameter Graphite [67] Bilayer [76] Bilayer [55] Bilayer [56] Bilayer [80] Trilayer [82]

γ0 3.16(5) 2.9 3.0a - 3.16(3) 3.1a

γ1 0.39(1) 0.30 0.40(1) 0.404(10) 0.381(3) 0.39a

γ2 -0.020(2) - - - - -0.028(4)

γ3 0.315(15) 0.10 0.3a - 0.38(6) 0.315a

γ4 0.044(24) 0.12 0.15(4) - 0.14(3) 0.041(10)

γ5 0.038(5) - - - - 0.05(2)

∆ -0.008(2) - 0.018(3) 0.018(2) 0.022(3) -0.03(2)

∆′ 0.050(6) - 0.018(3) 0.018(2) 0.022(3) 0.046(10)

a This parameter was not determined by the given experiment, the value quoted was taken from previous literature.

Bernal-stacked trilayer graphene by observation of Lan-dau level crossings [82]. Note that there are seven param-eters in the Slonczewski-Weiss-McClure (SWM) model ofgraphite [64–67] because the next-nearest layer couplingsγ2 and γ5, absent in bilayer, are present in graphite (andtrilayer graphene, too). Parameter ∆ in the SWM modelis related by ∆ = ∆′+γ2−γ5 to the parameter ∆′ describ-ing the energy difference between dimer and non-dimersites in bilayer graphene.

The energy bands are plotted in figure 3 along thekx axis in reciprocal space intersecting the corners K−,K+ and the centre Γ of the Brillouin zone [see fig-ure 1(b)]. Plots were made using Hamiltonian Hb, equa-tion (16), with parameter values determined by infraredspectroscopy γ0 = 3.16 eV, γ1 = 0.381 eV, γ3 = 0.38 eV,γ4 = 0.14 eV, ǫB1 = ǫA2 = ∆′ = 0.022 eV, and ǫA1 =ǫB2 = U = δAB = 0 [80]. There are four bands becausethe model takes into account one 2pz orbital on each ofthe four atomic sites in the unit cell; a pair of conduc-tion bands and a pair of valence bands. Over most ofthe Brillouin zone, each pair is split by an energy of theorder of the interlayer spacing γ1 ≈ 0.4 eV [83]. Nearthe K points, inset of figure 3, one conduction band andone valence band are split away from zero energy by anenergy of the order of the interlayer coupling γ1, whereastwo bands touch at zero energy [9]. The ‘split’ bands area bonding and anti-bonding pair arising from the strongcoupling (by interlayer coupling γ1) of the orbitals on thedimer B1 and A2 sites, whereas the ‘low-energy’ bandsarise from hopping between the non-dimer A1 and B2sites. In pristine bilayer graphene, the Fermi level lies atthe point where the two low-energy bands touch (shownas zero energy in figure 3) and, thus, this region is rele-vant for the study of electronic properties. It will be thefocus of the following sections.

At low energy, the shape of the band structure pre-dicted by the tight-binding model (see inset in figure 3) isin good agreement with that calculated by density func-tional theory [18, 57, 68] and it is possible obtain valuesfor the tight-binding parameters in this way, generally

E(eV)

Γ K+

E(eV)

px

1.5

1.0

0.5

-1.5

-1.0

-0.5

K-

kx

-8

-6

-4

-2

2

4

6

8

FIG. 3. Low-energy bands of bilayer graphene arising from2pz orbitals plotted along the kx axis in reciprocal space in-tersecting the corners K−, K+ and the centre Γ of the Bril-louin zone. The inset shows the bands in the vicinity of theK+ point. Plots were made using Hamiltonian Hb, equa-tion (16), with parameter values γ0 = 3.16 eV, γ1 = 0.381 eV,γ3 = 0.38 eV, γ4 = 0.14 eV, ǫB1 = ǫA2 = ∆′ = 0.022 eV, andǫA1 = ǫB2 = U = δAB = 0 [80].

in line with the experimental ones listed in Table I. Thetight-binding model HamiltonianHb, equation (16), usedin conjuction with the parameters listed in Table I, is notaccurate over the whole Brillouin zone because the fittingof tight-binding parameters is generally done in the vicin-ity of the corners of the Brillouin zone K+ and K− (asthe Fermi level lies near zero energy). For example, pa-rameter s0 in equation (28) describing non-orthogonalityof adjacent orbitals has been neglected here, but it con-tributes electron-hole asymmetry which is particularlyprevalent near the Γ point at the centre of the Brillouinzone [53, 60].

7

4. Effective four-band Hamiltonian near the K points

To describe the properties of electrons in the vicinity ofthe K points, a momentum p = ~k− ~Kξ is introducedwhich is measured from the centre of the Kξ point. Ex-panding in powers of p, the function f(k), equation (12),

is approximately given by f(k) ≈ −√3a(ξpx − ipy)/2~

which is valid close to the Kξ point, i.e., for pa/~ ≪ 1,

where p = |p| = (p2x + p2y)1/2. In monolayer graphene,

the Hamiltonian matrix (13) is simplified by keeping onlylinear terms in momentum p as

Hm =

(

ǫA vπ†

vπ ǫB

)

, (29)

where π = ξpx + ipy, π† = ξpx − ipy, and v =

√3aγ0/2~

is the band velocity. In the intrinsic case, ǫA = ǫB = 0,the eigen energy becomes E = ±v|p|, which approxi-mates Eq. (15). In bilayer graphene, similarly, Eq. (16)is reduced to

Hb =

ǫA1 vπ† −v4π† v3π

vπ ǫB1 γ1 −v4π†

−v4π γ1 ǫA2 vπ†

v3π† −v4π vπ ǫB2

, (30)

where we introduced the effective velocities, v3 =√3aγ3/2~ and v4 =

√3aγ4/2~.

At zero magnetic field Hamiltonian (30) yields fourvalley-degenerate bands E(p). A simple analytic solutionmay be obtained by neglecting the terms v4π, v4π

† pro-portional to γ4, and by considering only interlayer asym-metry U in the on-site energies: ǫA1 = ǫB1 = −U/2 andǫA2 = ǫB2 = U/2. Then, there is electron-hole symme-try, i.e., energies may be written E = ±εα(p), α = 1, 2,[9] with

ε2α =γ212

+U2

4+

(

v2 +v232

)

p2 + (−1)α√Γ , (31)

Γ = 14

(

γ21 − v23p2)2

+ v2p2[

γ21 + U2 + v23p2]

+ 2ξγ1v3v2p3 cos 3ϕ ,

where ϕ is the polar angle of momentum p = (px, py) =p (cosϕ, sinϕ). Energy ε2 describes the higher-energybands split from zero energy by the interlayer couplingγ1 between the orbitals on the dimer sites B1, A2.Low-energy bands E = ±ε1 are related to orbitals on

the non-dimer sites A1, B2. In an intermediate energyrange U, (v3/v)

2γ1 < ε1 < γ1 it is possible to neglectthe interlayer asymmetry U and terms proportional toγ3 (i.e., set U = v3 = 0), and the low-energy bands maybe approximated [9] as

ε1 ≈ 12γ1

[

√

1 + 4v2p2/γ21 − 1

]

, (32)

which interpolates between an approximately linear dis-persion ε1 ≈ vp at large momentum to a quadratic oneε1 ≈ p2/2m at small momentum, where the mass is

m = γ1/2v2 (see inset in figure 3). This crossover oc-

curs at p ≈ γ1/2v. A convenient way to describe thebilayer at low energy and momentum p ≪ γ1/2v is toeliminate the components in the Hamiltonian (30) re-lated to the orbitals on dimer sites B1, A2, resulting inan effective two-component Hamiltonian describing theorbitals on the non-dimer sites A1, B2, and, thus, thetwo bands that approach each other at zero energy. Thisis described in the next section, and the solutions of thisHamiltonian are shown to be massive chiral quasiparti-cles [8, 9], as opposed to massless chiral ones in monolayergraphene.

C. Effective two-band Hamiltonian at low energy

In this section we focus on the low-energy electronicband structure in the vicinity of the points K+ and K−at the corners of the first Brillouin zone, relevant for en-ergies near the Fermi level. A simple model may be ob-tained by eliminating orbitals related to the dimer sites,resulting in an effective Hamiltonian for the low-energyorbitals. First, we outline the procedure in general terms,because it may be applied to systems other than bilayergraphene such as ABC-stacked (rhombohedral) graphenemultilayers [84, 85], before applying it specifically to bi-layer graphene.

1. General procedure

We consider the energy eigenvalue equation, and con-sider separate blocks in the Hamiltonian corresponding to

low-energy θ = (ψA1, ψB2)Tand dimer χ = (ψA2, ψB1)

T

components:

(

hθ u

u† hχ

)(

θ

χ

)

= E

(

θ

χ

)

, (33)

The second row of (33) allows the dimer components tobe expressed in terms of the low-energy ones:

χ = (E − hχ)−1u†θ , (34)

Substituting this into the first row of (33) gives an effec-tive eigenvalue equation written solely for the low-energycomponents:

[

hθ + u (E − hχ)−1 u†

]

θ = Eθ ,[

hθ − uh−1χ u†

]

θ ≈ ESθ ,

where S = 1 + uh−2χ u†. The second equation is accurate

up to linear terms in E. Finally, we perform a transfor-mation Φ = S1/2θ:

[

hθ − uh−1χ u†

]

S−1/2Φ ≈ ES1/2Φ ,

S−1/2[

hθ − uh−1χ u†

]

S−1/2Φ ≈ EΦ . (35)

8

This transformation ensures that normalisation of Φ isconsistent with that of the original states:

Φ†Φ = θ†Sθ = θ†(

1 + uh−2χ u†

)

θ ,

≈ θ†θ + χ†χ ,

where we used equation (34) for small E: χ ≈ −h−1χ u†θ.

Thus, the effective Hamiltonian for low-energy compo-nents is given by equation (35):

H(eff) ≈ S−1/2[

hθ − uh−1χ u†

]

S−1/2 , (36)

S = 1 + uh−2χ u† . (37)

2. Bilayer graphene

The Hamiltonian (30) is written in basisA1, B1, A2, B2. If, instead, it is written inthe basis of low-energy and dimer components(θ, χ) ≡ A1, B2, A2, B1, equation (33), then

hθ =

(

ǫA1 v3π

v3π† ǫB2

)

, hχ =

(

ǫA2 γ1γ1 ǫB1

)

,

u =

(

−v4π† vπ†

vπ −v4π

)

, u† =

(

−v4π vπ†

vπ −v4π†

)

.

Using the procedure described in the previous section,equations (36,37), it is possible to obtain an effective

Hamiltonian H(eff) ≡ H2 for components (ψA1, ψB2). Anexpansion is performed by assuming that the intralayerhopping γ0 and the interlayer coupling γ1 are larger thanother energies: γ0, γ1 ≫ |E|, vp, |γ3|, |γ4|, |U |, |∆′|, |δAB|.Then, keeping only terms that are linear in the smallparameters |γ3|, |γ4|, |U |, |∆′|, |δAB| and quadratic in mo-mentum, the effective Hamiltonian [9, 63] is

H2 = h0 + hw + h4 + h∆ + hU + hAB, (38)

h0 = − 1

2m

(

0(

π†)2

π2 0

)

,

hw = v3

(

0 π

π† 0

)

− v3a

4√3~

(

0(

π†)2

π2 0

)

,

h4 =2vv4γ1

(

π†π 0

0 ππ†

)

,

h∆ =∆′v2

γ21

(

π†π 0

0 ππ†

)

,

hU = −U2

[(

1 0

0 −1

)

− 2v2

γ21

(

π†π 0

0 −ππ†

)]

,

hAB =δAB

2

(

1 0

0 −1

)

,

where π = ξpx + ipy, π† = ξpx − ipy. In the following

sections, we discuss the terms in H2. The first term h0

describes massless chiral electrons, section IID. It gener-ally dominates at low energy |E| ≪ γ1, so that the other

terms in H2 may be considered as perturbations of it.

The second term hw, section II E, introduces a triangu-lar distortion of the Fermi circle around each K point

known as ‘trigonal warping’. Terms hU and hAB, with±1 on the diagonal, produce a band gap between the

conduction and valence bands, section IIG, whereas h4and h∆ introduce electron-hole asymmetry into the bandstructure, section II F.The Hamiltonian (38) is written in the vicinity of a

valley with index ξ = ±1 distinguishing between K+ andK−. In order to briefly discuss the effect of symmetry op-erations on it, we introduce Pauli spin matrices σx, σy, σzin the A1/B2 sublattice space and Πx, Πy, Πz in the val-ley space. Then, the first term in the Hamiltonian may be

written as h0 = −(1/2m)[σx(p2x−p2y)+2Πzσypxpy]. The

operation of spatial inversion i is represented by Πxσxbecause it swaps both valleys and lattice sites, time inver-sion is given by complex conjugation and Πx, as it swapsvalleys, too. Hamiltonian (38) satisfies time-inversionsymmetry at zero magnetic field. The intrinsic terms

h0, hw, h4, and h∆ satisfy spatial-inversion symmetrybecause the bilayer crystal structure is spatial-inversion

symmetric, but terms hU and hAB, with ±1 on the di-agonal, are imposed by external fields and they violatespatial-inversion symmetry, producing a band gap be-tween the conduction and valence bands.

D. Interlayer coupling γ1: massive chiral electrons

The Hamiltonian h0 in equation (38) resembles theDirac-like Hamiltonian of monolayer graphene, butwith a quadratic-in-momentum term on the off-diagonalrather than linear. For example, the term π2/2m ac-counts for an effective hopping between the non-dimersites A1, B2 via the dimer sites B1, A2 consisting of ahop from A1 to B1 (contributing a factor vπ), followed bya transition between B1, A2 dimer sites (giving a ‘mass’∼ γ1), and a hop from A2 to B2 (a second factor of vπ).The solutions are massive chiral electrons [8, 9], withparabolic dispersion E = ±p2/2m, m = γ1/2v

2. Thedensity of states is m/(2π~2) per spin and per valley, andthe Fermi velocity vF = pF /m is momentum dependent,unlike the Fermi velocity v of monolayer graphene.The corresponding wave function is given by

ψ =1√2

(

1

∓e2iξϕ

)

eip.r/~ . (39)

The wave function components describe the electronicamplitudes on the A1 and B2 sites, and it can be usefulto introduce the concept of a pseudospin degree of free-dom [8, 9] that is related to these amplitudes. If all theelectronic density were located on the A1 sites, then thepseudospin part of the wave function |↑〉 = (1, 0) could beviewed as a pseudospin ‘up’ state, pointing upwards out

9

of the graphene plane. Likewise, a state |↓〉 = (0, 1) withdensity solely on the B2 sites could be viewed as a pseu-dospin ‘down’ state. However, density is usually sharedequally between the two layers, so that the pseudospinis a linear combination of up and down, |↑〉 ∓ e2iξϕ|↓〉,equation (39), and it lies in the graphene plane.

The Hamiltonian may also be written as h0 =(p2/2m)σ.n2 where the pseudospin vector is σ =(σx, σy, σz), and n2 = − (cos 2ϕ, ξ sin 2ϕ, 0) is a unit vec-tor. This illustrates the chiral nature of the electrons[8, 9]: the chiral operator σ.n2 projects the pseudospinonto the direction of quantization n2, which is fixed to liein the graphene plane, but turns twice as quickly as themomentum p. For these chiral quasiparticles, adiabaticpropagation along a closed orbit produces a Berry’s phase[86] change of 2π [8, 9] of the wave function, in contrastto Berry phase π in monolayer graphene.

Note that the chiral Hamiltonian h0 may be viewed as ageneralisation of the Dirac-like Hamiltonian of monolayergraphene and the second (after the monolayer) in a familyof chiral Hamiltonians HJ , J = 1, 2, . . ., corresponding toBerry’s phase Jπ which appear at low energy in ABC-stacked (rhombohedral) multilayer graphene [9–15, 84,85]:

HJ = gJ

(

0(

π†)J

πJ 0

)

, (40)

where g1 = v for monolayer, g2 = −1/2m for bilayer, andg3 = v3/γ21 for trilayer graphene. Since the pseudospin isrelated to the wavefunction amplitude on sites that arelocated on different layers, pseudospin may be viewed asa ‘which layer’ degree of freedom [14, 87].

E. Interlayer coupling γ3: trigonal warping and the

Lifshitz transition

The Hamiltonian h0 in equation (38) yields aquadratic, isotropic dispersion relation E = ±p2/2mwith circular iso-energetic lines, i.e., there is a circularFermi line around each K point. This is valid near theK point, pa/~ ≪ 1, whereas, at high energy, and mo-mentum p far from the K point, there is a triangularperturbation of the circular iso-energetic lines known astrigonal warping, as in monolayer graphene and graphite.It occurs because the band structure follows the symme-try of the crystal lattice as described by the full momen-tum dependence of the function f(k), equation (12) [88].In bilayer graphene [9], as in bulk graphite [89–92], a

second source of trigonal warping arises from the skew in-terlayer coupling γ3 between non-dimer A1 and B2 sites.The influence of γ3 on the band structure is describedby equation (31). In the two-band Hamiltonian, it is

described by hw in equation (38), the second term ofwhich arises from a quadratic term in the expansion off(k) ≈ −

√3a(ξpx − ipy)/2~+ a2(ξpx + ipy)

2/8~2. This

second term has the same momentum dependence as h0,

and, thus, it actually only gives a small additional con-

tribution to the mass m. The first term in hw causestrigonal warping of the iso-energetic lines in directionsϕ = ϕ0, where ϕ0 = 0, 23π,

43π at K+, ϕ0 = 1

3π, π,53π at

K−.

To analyse the influence of hw at low energy, we con-

sider just h0 and the first term in hw, and the resultingenergy E = ±ε1 is given by

ε21 = (v3p)2 − ξv3p

3

mcos (3ϕ) +

(

p2

2m

)2

, (41)

in agreement with equation (31) for U = 0, vp/γ1 ≪1, and v3/v ≪ 1. As it is linear in momentum, the

influence of hw and the resulting triangular distortionof iso-energetic lines tend to increase as the energy andmomentum are decreased until a Lifshitz transition [93]occurs at energy

εL =γ14

(v3v

)2

≈ 1meV. (42)

For energies |E| < εL, iso-energetic lines are broken intofour separate ‘pockets’ consisting of one central pocketand three ‘leg’ pockets, the latter centred at momentump ≈ γ1v3/v

2 and angle ϕ0, as shown in Figure 4. Thecentral pocket is approximately circular for |E| ≪ εLwith area Ac ≈ πε2/(~v3)

2, while each leg pocket is ap-proximately elliptical with area Al ≈ Ac/3. Note thatBerry phase 2π is conserved through the Lifshitz transi-tion; the three leg pockets each have Berry phase π whilethe central pocket has −π [12, 94].

F. Interlayer coupling γ4 and on-site parameter ∆′:

electron-hole asymmetry

Skew interlayer coupling γ4 between a non-dimer anda dimer site, i.e., between A1 and A2 sites or between

B1 and B2 sites, is described by h4 in equation (38),

where the effective velocity is v4 =√3aγ4/2~. This term

produces electron-hole asymmetry in the band struc-ture, as illustrated by considering the energy eigenvalues

E = ±(p2/2m)(1 ± 2v4/v) of the Hamiltonian h0 + h4.The energy difference ∆′ between dimer and non-dimersites, ǫA1 = ǫB2 = 0, ǫB1 = ǫA2 = ∆′, equation (26),also introduces electron-hole asymmetry into the band

structure: the low-energy bands described by h0 + h∆are given by E = ±p2/2m(1±∆′/γ1).

G. Asymmetry between on-site energies: band

gaps

1. Interlayer asymmetry

Interlayer asymmetry U , equation (25), describes a dif-ference in the on-site energies of the orbitals on the two

10

-2 -1 0 1 2-2

-1

0

1

2

px / pL

py /

pL

px / pL

py / pL

E / εL

55

1010

1515

2020

2525

FIG. 4. (a) Trigonal warping of the equi-energy lines in thevicinity of each K point, and the Lifshitz transition in bilayergraphene. The energy is in units of εL. (b) Correspondingthree-dimensional plot of the low-energy dispersion.

layers ǫA1 = ǫB1 = −ǫA2 = −ǫB2 = −U/2. Its influenceon the bands E = ±εα(p) is described by equation (31)with v3 = 0:

ε2α =γ212

+U2

4+ v2p2 + (−1)

α

√

γ414

+ v2p2 [γ21 + U2] ,

(43)

The low-energy bands, α = 1, display a distinctive ‘Mex-ican hat’ shape with a band gap Ug between the conduc-tion and valence bands which occurs at momentum pgfrom the centre of the valley:

Ug =|U |γ1

√

γ21 + U2; pg =

|U |2v

√

2γ21 + U2

γ21 + U2. (44)

For small values of the interlayer asymmetry U , the bandgap is equal to the asymmetry Ug = |U |, but for largeasymmetry values |U | ≫ γ1 the band gap saturatesUg → γ1. It is possible to induce interlayer asymme-try in bilayer graphene through doping [16] or the use ofexternal gates [17, 19, 20]. This is described in detail insection III.

2. Intralayer asymmetry between A and B sites

The energy difference δAB between A and B sites maybe described by the Hamiltonian (30) with ǫA1 = −ǫB1 =ǫA2 = −ǫB2 = δAB/2 and v3 = v4 = 0, yielding bandsE = ±εα:

ε2α =δ2AB

4+γ214

[

√

1 + 4v2p2/γ21 + (−1)α]2

. (45)

Thus, δAB creates a band gap, but there is no Mexicanhat structure.

H. Next-nearest neighbour hopping

The terms described in Hamiltonians (16,30,38) do notrepresent an exhaustive list of all possibilities. Addi-tional coupling parameters may be taken into account.For example, next-nearest neighbour hopping within eachlayer [95–98] results in a term (3 − |f(k)|2)γn appear-ing on every diagonal element of the Hamiltonian (16),where γn is the coupling parameter between next-nearestA (or B sites) on each layer. Ignoring the constant-in-momentum part 3γn produces an additional term in thetwo-component Hamiltonian (38)

hn = −γnv2p2

γ20

(

1 0

0 1

)

,

resulting in energies E = ±p2/2m(1 ∓ γnγ1/γ20).

Thus, next-nearest neighbour hopping represents another

source of electron-hole asymmetry, after h4, h∆, and Sb.

I. Spin-orbit coupling

For monolayer graphene, Kane and Mele [99] employeda symmetry analysis to show that there are two distincttypes of spin-orbit coupling at the corners K+ and K− ofthe Brillouin zone. These two types of spin-orbit couplingexist in bilayer graphene, too. In both monolayers andbilayers, the magnitude of spin-orbit coupling - althoughthe subject of theoretical debate - is generally consideredto be very small, with estimates roughly in the range of1 to 100µeV [99–109].At the corner of the Brillouin zone Kξ in bilayer

graphene, the contribution of spin-orbit coupling to thetwo-component low-energy Hamiltonian (38) may bewritten as

hSO = λSOξσzSz , (46)

hR = λR (ξσxSy + σySx) , (47)

where σi, i = x, y, z are Pauli spin matrices in the A1/B2sublattice space, and Sj , j = x, y, z are Pauli spin ma-

trices in the spin space. The first term hSO is intrin-sic to graphene, i.e. it is a full invariant of the sys-

tem. Both intra- and inter-layer contributions to hSO

11

have been discussed [105–107, 109] with the dominantcontribution to its magnitude λSO attributed to skewinterlayer coupling between π and σ orbitals [106, 107]or to the presence of unoccupied d orbitals within each

graphene layer [109]. Taken with the quadratic term h0in the Hamiltonian (38), hSO produces a gap of magni-tude 2λSO in the spectrum of bilayer graphene, but thetwo low-energy bands remain spin and valley degenerate(as in a monolayer): E = ±

√

λ2SO + v4p4/γ21 . However,there are gapless edge excitations and, like monolayergraphene [99], bilayer graphene in the presence of intrin-sic spin-orbit coupling is a topological insulator with afinite spin Hall conductivity [110, 111].The second type of spin-orbit coupling is the Bychkov-

Rashba term hR, equation (47), which is permitted only ifmirror reflection symmetry with respect to the grapheneplane is broken, by the presence of an electric field ora substrate, say [99–101, 105, 110–116]. Taken with the

quadratic term h0 in the Hamiltonian (38), hR does notproduce a gap, but, as in the monolayer, spin-splittingof magnitude 2λR between the bands. That is, there arefour valley-degenerate bands at low energy,

E2 = λ2R

(√

1 +v4p4

λ2Rγ21

± 1

)2

. (48)

Generally speaking, there is a rich interplay betweentuneable interlayer asymmetry U and the influence of theintrinsic and the Bychkov-Rashba spin-orbit coupling inbilayer graphene [105, 110, 111, 115, 116]. For example,the presence of interlayer asymmetry U breaks inversionsymmetry and allows for spin-split levels in the presenceof intrinsic spin-orbit coupling only (λR = 0) [105], whilethe combination of finite U and very large Rashba cou-pling has been predicted to lead to a topological insulatorstate even with λSO = 0 [115].

J. The integer quantum Hall effect

When a two-dimensional electron gas is placed in aperpendicular magnetic field, electrons follow cyclotronorbits and their energies are quantised as Landau levels[117]. At a high enough magnetic field strength, the dis-crete nature of the Landau level spectrum is manifest asthe integer quantum Hall effect [118–120], whereby theHall conductivity assumes values that are integer multi-ples of the quantum of conductivity e2/h.The Landau level spectrum of monolayer graphene was

calculated by McClure [121] nearly sixty years ago, andthere have been a number of related theoretical studies[5, 6, 98, 122–124] considering the consequences of chi-rality in graphene. The experimental observation of theinteger quantum Hall effect in monolayer graphene [2, 3]found an unusual sequencing of the quantised plateausof Hall conductivity, confirming the chiral nature of theelectrons and prompting an explosion of interest in the

field [7]. In bilayer graphene, the observation of the in-teger quantum Hall effect [8] and the calculated Landaulevel spectrum [9] uncovered additional features relatedto the chiral nature of the electrons.

1. The Landau level spectrum of bilayer graphene

We consider the Landau level spectrum of the two-

component chiral Hamiltonian h0, equation (38). Themagnetic field is accounted for by the operator p =(px, py) ≡ −i~∇+eA whereA is the vector potential andthe charge of the electron is −e. For a magnetic field per-pendicular to the bilayer, B = (0, 0,−B) where B = |B|,the vector potential may be written in the Landau gaugeA = (0,−Bx, 0), which preserves translational invari-ance in the y direction. Then, π = −i~ξ∂x + ~∂y − ieBxand π† = −i~ξ∂x−~∂y + ieBx, and eigenstates are com-prised of functions that are harmonic oscillator statesin the x direction and plane waves in the y direction[119, 120],

φℓ (x, y) = Aℓ Hℓ

(

x

λB− pyλB

~

)

exp

[

−1

2

(

x

λB− pyλB

~

)2

+ ipyy

~(49)

where the magnetic length is λB =√

~/eB, Hℓ areHermite polynomials of order ℓ for integer ℓ ≥ 0, and

Aℓ = 1/√

2ℓℓ!√π is a normalisation constant.

The operators π and π† appearing in the Hamilto-nian (38) act as raising and lowering operators for theharmonic oscillator states (49). At the first valley, K+,

K+ : πφℓ = −√2i~

λB

√ℓ φℓ−1 , (50)

K+ : π†φℓ =

√2i~

λB

√ℓ+ 1φℓ+1 , (51)

and πφ0 = 0. Then, it is possible to show that the Lan-dau level spectrum of the Hamiltonian (38) consists of aseries of electron and hole levels with energies and wavefunctions [9] given by

Eℓ,± = ±~ωc

√

ℓ(ℓ− 1) , ℓ ≥ 2, (52)

K+ : ψℓ,± =1√2

(

φℓ±φℓ−2

)

, ℓ ≥ 2, (53)

where ωc = eB/m and ± refer to the electron and holestates, respectively. For high values of the index, ℓ ≫ 1,the levels are approximately equidistant with spacing ~ωc

proportional to the magnetic field strength B. However,this spectrum, equation (52), is only valid for sufficientlysmall level index and magnetic field ℓ~ωc ≪ γ1 becausethe effective Hamiltonian (38) is only applicable at lowenergy.In addition to the field-dependent levels, there are two

levels fixed at zero energy E1 = E0 = 0 with eigenfunc-tions:

K+ : ψ1 =

(

φ10

)

, ψ0 =

(

φ00

)

, (54)

12

They may be viewed as arising from the square of thelowering operator in the Hamiltonian (38) which acts onboth the oscillator ground state and the first excited stateto give zero energy π2φ0 = π2φ1 = 0. The eigenfunctionsψ0 and ψ1 have a finite amplitude on the A1 sublattice,on the bottom layer, but zero amplitude on the B2 sub-lattice.At the second valley, K−, the roles of operators π and

π† are reversed:

K− : πφℓ = −√2i~

λB

√ℓ+ 1φℓ+1 , (55)

K− : π†φℓ =

√2i~

λB

√ℓ φℓ−1 , (56)

and π†φ0 = 0. The Landau level spectrum at K− is

degenerate with that at K+, i.e., Eℓ,± = ±~ωc

√

ℓ(ℓ− 1)for ℓ ≥ 2 and E1 = E0 = 0, but the roles of the A1 andB2 sublattices are reversed:

K− : ψℓ,± =1√2

(

φℓ−2

±φℓ

)

, ℓ ≥ 2, (57)

K− : ψ1 =

(

0

φ1

)

, ψ0 =

(

0

φ0

)

, (58)

The valley structure and electronic spin each contribute atwofold degeneracy to the Landau level spectrum. Thus,each level in bilayer level graphene is fourfold degenerate,except for the zero energy levels which have eightfolddegeneracy due to valley, spin and the orbital degeneracyof ψ0, ψ1.

2. Three types of integer quantum Hall effect

The form of the Landau level spectrum is manifest ina measurement of the integer quantum Hall effect. Here,we will compare the density dependence of the Hall con-ductivity σxy(n) for bilayer graphene with that of a con-ventional semiconductor and of monolayer graphene.The Landau level spectrum of a conventional two-

dimensional semiconductor is Eℓ = ~ωc(ℓ + 1/2), ℓ ≥ 0,where ωc = eB/m is the cyclotron frequency [119, 120].As density is changed, there is a step in σxy whenever aLandau level is crossed, and the separation of steps onthe density axis is equal to the maximum carrier den-sity per Landau level, gB/ϕ0, where ϕ0 = h/e is theflux quantum and g is a degeneracy factor. Each plateauof the Hall conductivity σxy occurs at a quantised valueof Nge2/h where N is an integer labelling the plateauand g is an integer describing the level degeneracy; stepsbetween adjacent plateaus have height ge2/h.The Landau level spectrum of monolayer graphene

[98, 121–124] consists of an electron and a hole series of

levels, Eℓ,± = ±√2ℓ~v/λB for ℓ ≥ 1, with an additional

level at zero energy E0 = 0. All of the levels are fourfolddegenerate, due to spin and valley degrees of freedom.

- 2

- 3

- 4

s x y ( 4 e2 / h )

1

2

3

4

- 11 2 3 4- 1- 2- 3- 4

- 2

- 3

- 4

s x y ( 4 e2 / h )

1

2

3

4

- 11 2 3 4- 1- 2- 3- 4

n ( 4 B / j 0 )

( a ) ( b )

n ( 4 B / j 0 )

FIG. 5. Schematic of the dependence of the Hall conductiv-ity σxy on carrier density n for (a) monolayer graphene and(b) bilayer graphene, where ϕ0 = h/e is the flux quantumand B is the magnetic field strength. The dashed line in (b)shows the behaviour for a conventional semiconductor or bi-layer graphene in the presence of large interlayer asymmetryU (section II J 3) with fourfold level degeneracy due to spinand valley degrees of freedom.

The corresponding Hall conductivity is shown schemati-cally in figure 5(a). There are steps of height 4e2/h be-tween each plateau, as expected by consideration of theconventional case, but the plateaus occur at half-integervalues of 4e2/h instead of integer ones, as observed ex-perimentally [2, 3]. This is due to the existence of thefourfold-degenerate level E0 = 0 at zero energy, whichcontributes to a step of height 4e2/h at zero density.

For bilayer graphene, plateaus in the Hall conductiv-ity σxy(n), Fig. 5(b), occur at integer multiples of 4e2/h.This is similar to a conventional semiconductor with leveldegeneracy g = 4 arising from the spin and valley de-grees of freedom. Deviation from the conventional caseoccurs at low density. In the bilayer there is a step inσxy of height 8e2/h across zero density, accompanied bya plateau separation of 8B/ϕ0 in density [8, 9], arisingfrom the eightfold degeneracy of the zero-energy Lan-dau levels. This is shown as the solid line in Fig. 5(b),whereas, for a conventional semiconductor, there no stepacross zero density (the dashed line).

Thus, the chirality of charge carriers in monolayer andbilayer graphene give rise to four- and eight-fold degen-erate Landau levels at zero energy and to steps of heightof four and eight times the conductance quantum e2/h inthe Hall conductivity at zero density [2, 3, 8]. Here, wehave assumed that the degeneracy of the Landau levelsis preserved, i.e., any splitting of the levels is negligibleas compared to temperature and level broadening in anexperiment. The role of electronic interactions in bilayergraphene is described in section VIII, while we discussthe influence of interlayer asymmetry on the Landau levelspectrum and integer quantum Hall effect in the next sec-tion.

13

3. The role of interlayer asymmetry

The Landau level states, equations (53,57), have dif-ferent amplitudes on the lower (A1 sublattice) and up-per (B2 sublattice) layers, with the role of the sublatticesites swapped at the two valleys. Thus, interlayer asym-

metry U as described by the effective Hamiltonian hU ,equation (38), leads to a weak splitting of the valley de-generacy of the levels [9]:

Eℓ,± ≈ ±~ωc

√

ℓ(ℓ− 1) +ξU~ωc

2γ1. (59)

Such splitting is prominent for the zero-energy states [9],equations (54,58), because they only have non-zero am-plitude on one of the layers, depending on the valley:

E0 = −1

2ξU , (60)

E1 = −1

2ξU +

ξU~ωc

γ1. (61)

When the asymmetry is large enough, then the splittingU of the zero energy levels from each valley results ina sequence of quantum Hall plateaus at all integer val-ues of 4e2/h including a plateau at zero density [17], asobserved experimentally [20]. This behaviour is shownschematically as the dashed line in figure 5(b). The Lan-dau level spectrum in the presence of large interlayerasymmetry U has been calculated [125–128], includingan analysis of level crossings [128] and a self-consistentcalculation of the spectrum in the presence of an exter-nal gate [126, 127], generalising the zero-field procedureoutlined in the next section.

III. TUNEABLE BAND GAP

A. Experiments

A tuneable band gap in bilayer graphene was first ob-served with angle-resolved photoemission of epitaxial bi-layer graphene on silicon carbide [16], and the ability tocontrol the gap was demonstrated by doping with potas-sium. Since then, the majority of experiments probingthe band gap have used single or dual gate devices basedon exfoliated bilayer graphene flakes [19, 20]. The bandgap has now been observed in a number of different ex-periments including photoemission [16], magnetotrans-port [20], infrared spectroscopy [55, 78–80, 129, 130],electronic compressibility [131, 132], scanning tunnellingspectroscopy [133], and transport [19, 31, 134–139].The gap observed in optics [16, 55, 78–80, 129, 130] is

up to 250meV [129, 130], the value expected theoretically(as the gap should saturate at the value of the interlayercoupling γ1). Transport measurements show insulatingbehaviour [19, 31, 134–139], but, generally, not the hugesuppression of conductivity expected for a gap of thismagnitude, and this has been attributed to edge states

x=-Lb

x=Lt

-c0

2

c0

2

Vb

Vt

εb

εt

εr

σb0

σt0

σ1

σ2

FIG. 6. Schematic of bilayer graphene in the presence of ex-ternal gates located at x = −Lb and x = +Lt, with po-tentials Vb and Vt, which are separated from the bilayer bymedia of dielectric constants εb and εt, respectively. The bi-layer is modelled as two parallel conducting plates positionedat x = −c0/2 and +c0/2, separated by a region of dielectricconstant εr. The layers have change densities σ1 = −en1 andσ2 = −en2 corresponding to layer number densities n1 andn2. Charge densities σb0 and σt0 (dashed lines) arise from thepresence of additional charged impurities.

[140], the presence of disorder [141–143] or disorder andchiral charge carriers [144]. Broadly speaking, transportseems to occur through different mechanisms in differenttemperature regimes with thermal activation [31, 134–136, 138, 139] at high temperature (above, roughly, 2 to50K) and variable-range [19, 135–137, 139] or nearest-neighbour hopping [135, 138] at low temperature.

B. Hartree model of screening

External gates are generally used to control the den-sity of electrons n on a graphene device [1], but, in bi-layer graphene, external gates will also place the sepa-rate layers of the bilayer at different potential energiesresulting in interlayer asymmetry U = ǫ2 − ǫ1 (whereǫ1 = ǫA1 = ǫB1 = −U/2 and ǫ2 = ǫA2 = ǫB2 = U/2).Thus, changing the applied gate voltage(s) will tend totune both the density n and the interlayer asymmetryU , and, ultimately, the band gap Ug. The dependence ofthe band gap on the density Ug(n) relies on screening byelectrons on the bilayer. In the following, we describe asimple model [17, 18, 20, 55, 69, 71, 145, 146] that hasbeen developed to take into account screening using thetight-binding model and Hartree theory.

1. Electrostatics: asymmetry parameter, layer densities andexternal gates

We use the SI system of units, and the electronic chargeis −e where e > 0. The bilayer graphene device is mod-elled as two parallel conducting plates that are very nar-row in the x-direction, continuous and infinite in the y-z plane, positioned at x = −c0/2 and +c0/2, figure 6.Here, c0 is the interlayer spacing and we denote the di-electric constant of the interlayer space as εr (it doesn’tinclude the screening by π-band electrons that we are ex-plicitly modelling). Layer number densities are n1 and

14

n2, with corresponding change densities σ1 = −en1 andσ2 = −en2.We take into account the presence of a back gate and a

top gate, infinite in the y-z plane, located at x = −Lb andx = +Lt, with potentials Vb and Vt, which are separatedfrom the bilayer by media of dielectric constants εb andεt, respectively. It is possible to describe the presenceof additional charge near the bilayer - due to impurities,say - by introducing density nb0 on the back-gate sideand nt0 on the top-gate side. They correspond to chargedensities σb0 = enb0 and σt0 = ent0, assuming that nb0

and nt0 are positive for positive charge.Using Gauss’s Law, it is possible to relate the external

gate potentials and impurities concentrations to the layerdensities and the interlayer asymmetry [17, 60, 145, 147]:

n = n1 + n2 =ε0εbVbeLb

+ε0εtVteLt

+ nb0 + nt0 , (62)

U = − εtεr

c0LteVt +

e2c0ε0εr

(n2 − nt0) , (63)

where the field within the bilayer interlayer space is ap-proximately equal to U/(ec0). Equation (62) expressesthe total electron density n = n1+n2 in terms of the ex-ternal potentials, generalising the relation for monolayergraphene [1]. Note that the background densities nb0 andnt0 shift the effective values of the gate potentials Vb andVt. The second equation, for U , may be rewritten as

U = Uext + Λγ1(n2 − n1)

n⊥, (64)

Uext =ec02εr

(

εbLbVb −

εtLtVt

)

+ Λγ1(nb0 − nt0)

n⊥, (65)

where the characteristic density scale n⊥ and the dimen-sionless screening parameter Λ are

n⊥ =γ21

π~2v2, Λ =

c0e2γ1

2π~2v2ε0εr≡ c0e

2n⊥2γ1ε0εr

. (66)

Equation (64) relates the asymmetry parameter U to asum of its value, Uext, if screening were negligible plusa term accounting for screening. Parameter values γ1 =0.39eV and v = 1.0×106ms−1 give n⊥ = 1.1×1013cm−2.With interlayer spacing c0 = 3.35A and an estimate forthe dielectric constant of εr ≈ 1, then Λ ∼ 1, showingthat screening is relevant.

2. Calculation of individual layer densities

Through electrostatics, the asymmetry parameter Uis related to layer densities n1 and n2, equation (64).The densities n1 and n2 also depend on U because ofthe band structure of bilayer graphene. Analytical cal-culations are possible [17, 18, 145] if only the dominantinter-layer coupling γ1 is taken into account in the four-band Hamiltonian (30). Here we will use the two-bandmodel (38) with an explicit ultraviolet cutoff [18] when

integrating over the whole Brillouin zone. The simplifiedtwo-component Hamiltonian is

H2 ≈ −v2

γ1

(

0(

π†)2

π2 0

)

− U

2

(

1 0

0 −1

)

, (67)

Solutions to the energy eigenvalue equation H2ψ = Eψare given by

E = ±√

U2

4+v4p4

γ21, (68)

ψ =

√

E − U/2

2E

(

1

− v2p2

γ1(E−U/2)e2iξϕ

)

eip.r/~ . (69)

Layer densities are determined by integration over thecircular Fermi surface

n1(2) =2

π~2

∫

|ψA1(B2)(p)|2p dp , (70)

where a factor of four takes account of spin and valleydegeneracy.For simplicity, we assume the Fermi energy lies within

the conduction band. Using the solution (69), the contri-bution of the partially-filled conduction band to the layerdensities [17, 145, 148] is given by

ncb1(2) =

1

π~2

∫

pdp

(

E ∓ U/2

E

)

, (71)

=1

π~2

∫ pF

0

pdp∓ U

2π~2

∫ pF

0

pdp√

U2/4 + v4p4/γ21,

≈ n

2∓ n⊥U

4γ1ln

2|n|γ1n⊥|U | +

√

1 +

(

2nγ1n⊥U

)2

,

where the minus (plus) sign is for the first (second) layer,pF is the Fermi momentum, and the total density is n =p2F /π~

2 measured with respect to the charge neutralitypoint, i.e., we assume that the point of zero density isrealised when the Fermi level lies at the crossing point ofthe conduction and valence bands.In addition, we take into account the contribution of

the filled valence band nvb1(2) to the individual layer den-

sities. Note that, as the asymmetry parameter U varies,the filled valence band does not contribute to any changein the total density n, but it does contribute to the dif-ference n1 − n2. This may be obtained by integratingwith respect to momentum as in equation (71), but in-troducing an ultraviolet cutoff pmax = γ1/v equivalentto nmax = n⊥ [18]. Then, the contribution of the filledvalence band [17, 18, 69, 71, 145, 146] is given by

nvb1(2) ≈ ± U

2π~2

∫ pmax

0

pdp√

U2/4 + v4p4/γ21,

≈ ±n⊥U

4γ1ln

(

4γ1|U |

)

. (72)

15

Combining the contributions of equations (71) and (72),the individual layer density, n1(2) = ncb

1(2)+nvb1(2), is given

[17, 145] by

n1(2)≈n

2∓n⊥U

4γ1ln

|n|2n⊥

+1

2

√

(

n

n⊥

)2

+

(

U

2γ1

)2

.(73)

Note that some calculations [148] include only the contri-bution (71) of the partially-filled conduction band, others[18] include only the filled valence band (72).

3. Self-consistent screening

Substituting the layer density (73) into the expres-sion (64) describing screening gives an expression [17,60, 145] for the density-dependence of the asymmetryparameter U :

U(n)

Uext≈

1− Λ

2ln

|n|2n⊥

+1

2

√

(

n

n⊥

)2

+

(

U

2γ1

)2

−1

(74)

where Uext is the asymmetry in the absence of screen-ing (65). The extent of screening is described by thelogarithmic term with argument depending on n andU , and a prefactor proportional to the screening pa-rameter Λ ∼ 1 (as discussed earlier). A common ex-perimental setup, especially for exfoliated graphene ona silicon substrate [1–3, 8], includes a single back gate.Figure 7 shows the density-dependence of the band gapUg(n) plotted as the back-gate voltage Vb is varied for afixed top-gate voltage Vt. In this case, the influence ofthe top-gate voltage Vt may be absorbed into an effec-tive offset-density n0 = 2[ε0εtVt/(eLt) + nt0] [17] givingUext = Λγ1(n − n0)/n⊥ in equation 74. Figure 8 showsthe dependence of the difference in layer densities n1−n2

for the case n0 = 0 including both the contribution ofthe partially filled bands as measured with respect tothe charge neutrality point (71) (dashed line) and thecontribution of the full valence band (72) (dotted line).The sum of both terms (solid line) shows that n1 − n2

is positive (negative) for positive (negative) total densityn. Recalling that layer 1 is closest to the back gate, thisshows that the bilayer is polarised along the electric field,as expected [145].A single back gate in the absence of additional charged

dopants may be described by Vt = nb0 = nt0 = 0, re-sulting in simplified expressions n = ε0εbVb/(eLb) (as inmonolayer graphene [1]) and Uext = Λγ1n/n⊥. Using|U | ≪ γ1, equation (74) simplifies [17, 60, 69, 71] as

U(n) ≈ Λγ1n

n⊥

[

1− Λ

2ln

( |n|n⊥

)]−1

, (75)

At high density |n| ∼ n⊥, the logarithmic term is neg-ligible and U(n) ≈ Λγ1n/n⊥ is approximately linear in

density. Note that the band gap Ug = |U |γ1/√

U2 + γ21

Ug/γ

1

n/n

1.0

0.8

0.6

0.2

0.4

0.5-0.5 1.0-1.0 0

n0/n

0.0

0.2

0.4

0.6

FIG. 7. Density-dependence of the band gap Ug(n) in bi-layer graphene as the back-gate voltage Vb is varied for afixed top-gate voltage Vt [17]. The effective offset-density isn0 = 2[ε0εtVt/(eLt) + nt0]. Plots were made for screening

parameter Λ = 1, using Ug = |U |γ1/√

U2 + γ21 and numerical

solution of equation (74).

n/n0.5-0.5 1.0-1.0

-0.4

0.2

0.4

-0.2

(n -n )/n1 2

FIG. 8. Density-dependence of the difference in layer densitiesn1 − n2 in bilayer graphene as the back-gate voltage Vb isvaried for a fixed top-gate voltage Vt [17]. Plots were madefor screening parameter Λ = 1 and the effective offset-densityis n0 = 2[ε0εtVt/(eLt) + nt0] = 0, corresponding to the datalabelled n0 = 0 in Figure 7, obtained by numerical solutionof equation (74). The dashed line shows the contributionof the partially filled bands as measured with respect to thecharge neutrality point (71) [148], the dotted line shows thecontribution of the full valence band (72) [18], the solid lineis their sum (73) [17, 145].

tends to saturate Ug → γ1, even if |U | ≫ γ1. At low den-sity, |n| ≪ n⊥, the logarithmic term describing screeningdominates and Ug ≈ |U | ≈ 2γ1(|n|/n⊥)/ ln(n⊥/|n|), in-dependent of the screening parameter Λ.The expressions (74,75) for U(n) take into account

screening due to low-energy electrons in pz orbitals usinga simplified Hamiltonian (67) while neglecting other or-bitals and the effects of disorder [55, 145, 149–155], crys-talline inhomogeneity [18] and electron-electron exchangeand correlation. Nevertheless, there is generally good

16

qualitative agreement of the dependence of U(n) on den-sity n predicted by equations (74,75) with density func-tional theory calculations [18, 73] and experiments in-cluding photoemission [16, 20] and infrared spectroscopy[55, 78–80, 129, 130]. Note that the Hartree screeningmodel has been generalised to describe graphene trilay-ers and multilayers [147, 156–158].

IV. TRANSPORT PROPERTIES

A. Introduction

Bilayer graphene exhibits peculiar transport proper-ties due to its unusual band structure, described in sec-tion II, where the conduction and valence bands touchwith quadratic dispersion. Transport characteristics andthe nature of conductivity near the Dirac point wereprobed experimentally [2, 3, 8, 19, 20, 159–162] and inves-tigated theoretically [163–175]. Neglecting trigonal warp-ing, the minimal conductivity is predicted to be 8e2/(πh)[163, 167, 168], twice the value in monolayer graphene,while, in the presence of trigonal warping, it is larger,24e2/(πh) [163, 169], because of multiple Fermi surfacepockets at low energy, section II E.For a detailed review of the electronic transport prop-

erties of graphene monolayer and bilayers, see Ref. [176,177]. The characteristics of bilayer graphene in the pres-ence of short-ranged defects and long-ranged charged-impurities have been calculated [54, 163, 164, 166, 171–175] and it is predicted that the conductivity has anapproximately linear dependence on density at typicalexperimental densities [172]. At interfaces and poten-tial barriers, conservation of the pseudospin degree offreedom may influence electronic transmission [178, 179],as in monolayer graphene [178, 180], including transmis-sion at monolayer-bilayer interfaces [181–184], throughmultiple electrostatic barriers [185], or magnetic barriers[186, 187]. Inducing interlayer asymmetry and a bandgap using an external gate [9, 17], described in section III,may be used to tune transport properties [181, 188]. In-terlayer asymmetry may also be viewed as creating anout-of-plane component of pseudospin and interfaces be-tween regions of opposite polarity have attracted theo-retical attention due to the existence of one-dimensionalvalley-polarised modes along the interface [189–192], apseudospintronic analogy of spin-valve devices for trans-port perpendicular to the interface [193, 194], electronicconfinement [195], and valley-dependent transmission[196].In the following we describe two different models of

the conductivity of bilayer graphene at low energy. Thefirst is for ballistic transport in a clean device of finitelength that is connected to semi-infinite leads, describedusing wave matching to calculate the transmission prob-ability and, then, the conductance. The second modeldescribes the conductivity of a disordered, infinite sys-tem using the Kubo formula and the self-consistent Born

L

W

x=Lx=0

FIG. 9. Two-probe bilayer graphene device with armchairedges, widthW and length L. The rectangular shaded regionsrepresent the ends of semi-infinite leads.

approximation to describe scattering from the disorderedpotential. Although the two models are quite different,both predict the minimal conductivity to be 8e2/(πh)[163, 167, 168]. Finally, in section IVC2, we describelocalisation effects.

B. Ballistic transport in a finite system

Ballistic transport in a finite, mesoscopic bilayergraphene nanostructure has been modelled in a numberof papers [165, 167–169, 178, 193, 194, 196]. Here, we fol-low a wave-matching approach of Snyman and Beenakker[168]. For bilayer, as compared to monolayer, there is anew length scale ℓ1 = ~v/γ1 characteristic of the inter-

layer coupling. Here, v =√3aγ0/2~ is the band velocity

of monolayer graphene, so ℓ1 = (√3/2)(γ0/γ1)a ≈ 18 A

is several times longer [168] than the lattice constanta = 2.46 A [53]. For most situations, the sample sizeL≫ ℓ1, and the device generally behaves as a (coupled)bilayer rather than two separate monolayers [168].We consider a two-probe geometry with armchair edges

as shown in Fig. 9. There is a central mesoscopic bilayerregion, width W and length L, connected to a left andright lead. This orientation is rotated by 90 as comparedto that described in section II so the corners of the Bril-louin zone are located at wavevectors Kξ = ξ(0, 4π/3a).In terms of wavevector measured from the centre of thevalley, i.e., ky → ky+ξ4π/3a, then the Hamiltonian (30)in basis A1, B1, A2, B2 may be written as

Hb =

U vπ† 0 0

vπ U γ1 0

0 γ1 U vπ†

0 0 vπ U

, (76)

where π = −i~(kx + iξky), π† = i~(kx − iξky), and U is

the on-site energy which describes the doping of the bi-layer. For simplicity, we include only the main interlayercoupling term γ1 of the orbitals on the dimer B1 and A2

17

sites. It is assumed that the transverse wavevector kyis real and it is conserved at the interfaces between thebilayer and the leads. The Hamiltonian (76) shows thereare two values of the longitudinal wavevector kx for givenU , ky and energy ε, which we denote as k+ and k−:

~vk± =√

(ε− U)2 ± γ1(ε− U)− ~2v2k2y . (77)

Left- ΦL± and right- ΦR

± moving wave functions may bewritten as

ΦL± = N±

∓i~v(−k± − iξky)

∓(ε− U)

(ε− U)

−i~v(−k± + iξky)

e−ik±x+ikyy , (78)

ΦR± = N±

∓i~v(k± − iξky)

∓(ε− U)

(ε− U)

−i~v(k± + iξky)

eik±x+ikyy , (79)

where normalisation N± = [4W (ε − U)k±]−1/2 for unit

current.

The aim is to describe a mesoscopic bilayer region offinite length L connected to macroscopic leads. In orderto mimick macroscopic, metallic contacts, there shouldbe many propagating modes in the leads that overlapwith the modes in the central bilayer region. If this isthe case, then the value of minimal conductance shouldnot depend on the particular model used for the leads,e.g., square lattice or graphene lattice, as demonstratedfor monolayer graphene [197]. Note, this will yield quitedifferent results from a model with a bilayer lead at thesame level of doping as the central region; then, the sys-tem is effectively an infinite system, not a finite, meso-scopic conductor.

Snyman and Beenakker [168] modelled the leads asheavily-doped bilayer graphene, generalising an approachdeveloped for monolayer graphene [198]. In this way,there are many conducting modes present in the leadsand it is possible to simply use matching of the bilayerwave functions at the interface between the central re-gion and the leads. In particular, the leads are mod-elled as bilayer graphene with on-site energy U = −U∞where U∞ > 0 and U∞ ≫ |ε|, γ1. Then, in the leads,k+ ≈ k− ≈ U∞/(~v) and wave functions ψleft,±, ψright,±,in the left (x < 0) and right (x > L) leads may be written

as

ψleft,± =

∓i∓1

1

−i

eiU∞x/~v + r±+

i

−1

1

i

e−iU∞x/~v

+ r±−

−i1

1

i

e−iU∞x/~v

eikyy , (80)

ψright,± =

t±+

−i−1

1

−i

+ t±−

i

1

1

−i

eiU∞(x−L)/~v+ikyy .

Here, a right-moving wave with unit flux correspond-ing to a state with wavevector k± ≈ U∞/(~v) is in-jected from the left lead [the first term in equation (80)].Subsequently, there are two left-moving waves that havebeen reflected with amplitudes r±+ and r±−, and two right-moving waves are transmitted to the right, with ampli-tudes t±+ and t±−.

At the charge-neutrality point ε = U = 0 in the centralbilayer region, the wave functions are evanescent withimaginary longitudinal wavevector, equation (77). Twostates with kx = −iξky have finite amplitude only on theA1, A2 sites and two with kx = iξky have finite amplitudeonly on the B1, B2 sites:

ψcentre,± =

c±1

1

0

0

0

eξkyy + c±2

γ1x/~v

0

1

0

eξkyy

+c±3

0

1

0

−γ1x/~v

e−ξkyy + c±4

0

0

0

1

e−ξkyy

eikyy .

For each incoming mode ± from the left lead [the firstterm in equation (80)], there are eight unknown ampli-tudes c±1 , c

±2 , c

±3 , c

±4 , r

±+ , r

±− , t

±+, t

±−. Continuity of the

wave functions at the interfaces x = 0 and x = L betweenthe central region and the leads provides eight simulta-

18

neous equations:

∓i+ ir±+ − ir±− = c±1 , (81)

∓1− r±+ + r±− = c±3 , (82)

1 + r±+ + r±− = c±2 , (83)

−i+ ir±+ + ir±− = c±4 , (84)

−it±+ + it±− = c±1 eξkyL + c±2

L

ℓ1eξkyL , (85)

−t±+ + t±− = c±3 e−ξkyL , (86)

t±+ + t±− = c±2 eξkyL , (87)

−it±+ − it±− = −c±3L

ℓ1e−ξkyL + c±4 e

−ξkyL , (88)

where ℓ1 = ~v/γ1. Solving yields the transmission matrix

t =

(

t++ t−+t+− t−−

)

=2i

2 + (L/ℓ1)2 + 2 cosh (2kyL)

×(

(L/ℓ1 − 2i) cosh (kyL) − (L/ℓ1) sinh (ξkyL)

(L/ℓ1) sinh (ξkyL) − (L/ℓ1 + 2i) cosh (kyL)

)

.

The transmission probability [168] is determined by theeigenvalues T± of the product tt†:

T± =1

cosh2 (ξkyL∓ kcL), (89)

kcL = ln

L

2ℓ1+

√

1 +

(

L

2ℓ1

)2

, (90)

The transmission coefficients T± have the same formas the transmission in monolayer graphene T =1/ cosh2(kyL) [198] but shifted by the parameter kc, asshown in figure 10.The conductance G may be determined using the

Landauer-Buttiker formula [199, 200]

G =gvgse

2

hTr(

tt†)

, (91)

where the factor of gvgs accounts for valley and spin de-generacy. For a short, wide sample whose width W ex-ceeds its length L, W ≫ L, the transverse wavevectormay be assumed to be continuous and

G =gvgse

2

h

W

2π

∫ ∞

−∞(T+ + T−) dky =

2gvgse2

h

W

πL.(92)

Thus, the minimal conductivity σ = GL/W = 8e2/(πh)is twice as large as in the monolayer. In a similar way, it ispossible to determine the Fano factor of shot noise whichtakes the same value 1/3 [168] as in monolayer graphene[198]. Transmission via evanescent modes in graphenehas been described as pseudodiffusive because the Fanofactor takes the same value as in a diffusive metal [198].

k Ly

T

FIG. 10. The transmission coefficients T± of bilayergraphene (89) for L = 50ℓ1 [168] (solid lines). The trans-mission coefficient of monolayer graphene [198] is shown inthe centre (dashed line).

C. Transport in disordered bilayer graphene

1. Conductivity

When the Fermi energy εF is much larger than the levelbroadening caused by the disorder potential, the systemis not largely different from a conventional metal, and theconductivity is well described by Boltzmann transporttheory. However, this approximation inevitably breaksdown at the Dirac point, where even the issue of whetherthe system is metallic or insulating is nontrivial. Tomodel electronic transport at the charge neutrality point,we need a refined approximation that properly includesthe finite level broadening. Here, we present a conduc-tivity calculation using the self-consistent Born approxi-mation (SCBA) [163]. We define the Green’s function asG(ε) = (ε − H)−1. The Green’s function averaged overthe impurity configurations satisfies the Dyson’s equation

〈Gα,α′(ε)〉 = δα,α′G(0)α (ε) + G(0)

α (ε)∑

α1

Σα,α1(ε)〈Gα1,α′(ε)〉,(93)

where 〈 〉 is an average over configurations of the disorderpotential, α is an eigenstate of the ideal Hamiltonian H0,

and G(0)α = (ε− εα)

−1, with εα being the eigenenergy ofthe state α in H0. In SCBA, the self-energy is given by[201]

Σα,α′(ε) =∑

α1,α′1

〈Uα,α1Uα′

1,α′〉〈Gα1,α′

1(ε)〉. (94)

The equations (93) and (94) need to be solved self-consistently. The conductivity is calculated using theKubo formula,

σ(ε) = gvgs~e2

2πΩReTr

[

vx〈GR〉vRAx 〈GA〉 − vx〈GR〉vRR

x 〈GR〉]

,

(95)

19

where GR = G(ε+ i0) and GA = G(ε− i0) are retardedand advanced Green’s functions, vx = ∂H0/∂px is thevelocity operator, and gvgs accounts for summation overvalleys and spins. vRA

x and vRRx the velocity operators

containing the vertex correction, defined by vRAx = vx(ε+

i0, ε− i0) and vRRx = vx(ε+ i0, ε+ i0) with

vx(ε, ε′) = vx + 〈UG(ε)vxG(ε′)U〉. (96)

In SCBA, vx should be calculated in the ladder approxi-mation.For the disorder potential, we assume a short-ranged

potential within each valley,

U =∑

i

uiδ(r− ri)

1 0 0 0

0 1 0 0

0 0 1 0

0 0 0 1

. (97)

and neglect intervalley scattering between K+ and K−.This situation is realized when the length scale of thescattering potential is larger than atomic scale but muchshorter than the Fermi wave length. We assume an equalamount of positive and negative scatterers ui = ±u anda total density of scatterers per unit area nimp.The SCBA formulation is applied to the low-energy

Hamiltonian equation (38), with the trigonal warping ef-fect due to γ3 included [163]. Energy broadening due tothe disorder potential is characterised by

Γ =π

2nimpu

2 m∗

2π~. (98)

When Γ>∼εL, i.e., the disorder is strong enough to smearout the fine band structure of the trigonal warping, wecan approximately solve the SCBA equation in an ana-lytic form. The self-energy, equation (94), becomes diag-onal with respect to index α and it is a constant,

Σ(ε+ i0) ≈ −iΓ. (99)

Then, the conductivity at the Fermi energy ε is writtenas

σ(ε) ≈ gvgse2

π2~

1

2

[

1 +

( |ε|Γ

+Γ

|ε|

)

arctan|ε|Γ

+4πεLΓ

]

.

(100)The third term in the square bracket arises from the ver-tex correction due to the trigonal warping effect, and εLis given by equation (42). For high energies |ε| ≫ Γ, σapproximates as

σ(ε) ≈ gvgse2

π2~

π

4

|ε|Γ, (101)

which increases linearly with energy. The value at zeroenergy becomes

σ(0) = gvgse2

π2~

(

1 +2πεLΓ

)

. (102)

-1 -0.5 0 0.5 10

2

4

6

8

-1 -0.5 0 0.5 10

5

10

15

20

25

DO

S

[in

units o

f g

vg

sm

*/2

πh

]

EF / γ

1

EF / γ

1

Conductivity

[in u

nits o

f g

vg

se

2/(

π2h)]

Γ / γ

1

0.15

0.015

0.03

0.08

Γ / γ

1

0.15

0.015

0.08

0.03

(a)

(b)

Ideal

FIG. 11. (a) Calculated density of states and (b) conductivityas a function of energy for different disorder strength Γ [202].In (b), broken curves show the results of the low-energy two-band model, and the horizontal line indicates the universalconductivity gvgse

2/(π2~).

In the strong disorder regime Γ ≫ 2πεL, the correctionarising from trigonal warping vanishes and the conductiv-ity approaches the universal value gvgse

2/(π2~) [163, 167]

which is twice as large as that in monolayer graphene inthe same approximation. In transport measurements ofsuspended bilayer graphene [161], the minimum conduc-tivity was estimated to be about 10−4S, which is close togvgse

2/(π2~).

The 2×2 (two-band) model works well at low energy,but it is not expected to be valid in the strong disorderregime when mixing to higher energy bands is consid-erable. To see this, we numerically solved SCBA equa-tion for the original 4×4 (four-band) Hamiltonian. Fig-ure 11(a) and (b) show the density of states (DOS) andconductivity, respectively, for several disorder strengths[202]. In (b) the results for the 2×2 model in equa-tion (100) are expressed as broken curves. In (a), weobserve that the DOS at zero energy is significantly en-hanced because states at high energies are shifted toward

20

the Dirac point by the disorder potential. However, thezero-energy conductivity barely shifts from that of the2×2 model [equation (102)], even for strong disorder suchas Γ/γ1 = 0.15, where the DOS at zero energy becomesnearly twice as large as in the 2×2 model. For higher en-ergy |ε| > Γ, the conductivity increases linearly with |ε|in qualitative agreement with equation (100) of the 2×2model, while the gradient is generally steeper. The con-ductivity has a small dip at the higher band edge around|ε| ∼ γ1, because the frequency of electron scattering isstrongly enhanced by the higher band states.The SCBA calculation was recently extended for long-

range scatterers [203]. It was shown that the conductivityat zero energy is not universal but depends on the degreeof disorder for scatterers with long-range potential, sim-ilar to monolayer graphene [204].

2. Localisation effects

The SCBA does not take account of some quantumcorrections, such as those included explicitly in weak lo-calisation. In graphene, the presence of spin-like degreesof freedom related to sublattices and valleys, as well asreal electronic spin itself, creates the possibility of a richvariety of quantum interference behaviour. Weak local-isation [205, 206] is a particularly useful probe becauseit is sensitive to elastic scattering that causes relaxationof the sublattice pseudospin and valley ‘spin’. In theabsence of symmetry-breaking scattering processes, con-servation of pseudospin in monolayer graphene tends tosuppress backscattering [88, 207], and the interference ofchiral electrons would be expected to result in antilocal-ization [208]. However, intravalley symmetry-breakingrelaxes the pseudospin and suppresses anti-localisation,while intervalley scattering tends to restore conventionalweak localisation [209–213], as observed experimentally[209, 214–219]. Nevertheless, anti-localisation has beenobserved at high temperature [218, 220] when the rel-ative influence of symmetry-breaking disorder is dimin-ished, and its presence has also been predicted at verylow temperature [221–223] when spin-orbit coupling mayinfluence the spin of the interfering electrons.In bilayer graphene, the pseudospin turns twice as

quickly in the graphene plane as in a monolayer, nosuppression of backscattering is expected and the quan-tum correction should be conventional weak localisation[212, 213, 224]. However, the relatively strong trigonalwarping of the Fermi line around each valley (describedin section II E) can suppress localisation unless interval-ley scattering is sufficiently strong [224]. Experimentalobservations confirmed this picture [159], and it was pos-sible to determine the temperature and density depen-dence of relevant relaxation lengths by comparing to thepredicted magnetoresistance formula [224].Localisation has also been studied for gapped bilayer

graphene in the presence of interlayer potential asymme-try U [225]. It was shown that, as long as the disorder

potential is long range and does not mix K± valleys, gapopening inevitably causes electron delocalisation some-where between U = 0 and U = ∞, in accordance withthe transition of quantum valley Hall conductivity, i.e.,the opposite Hall conductivities associated with two val-leys. This is an analog of quantum Hall physics but canbe controlled purely by an external electric field withoutany use of magnetic fields.

V. OPTICAL PROPERTIES

The electronic structure of bilayer graphene wasprobed by spectroscopic measurements in zero magneticfield [16, 55, 56, 79, 80, 129, 130], and also in high mag-netic fields [78]. The optical absorption for perpendic-ularly incident light is described by the dynamical con-ductivity in a electric field parallel to the layers, in bothsymmetric bilayers [164, 226–228] and in the presence ofan interlayer-asymmetry gap [227] For symmetric bilayergraphene, this is explicitly estimated as [164, 226–228]

Reσxx(ω) =gvgs16

e2

~

~ω + 2γ1~ω + γ1

θ(~ω − 2|εF |)

+( γ1~ω

)2

[θ(~ω − γ1) + θ(~ω − γ1 − 2|εF |)]

+~ω − 2γ1~ω − γ1

θ(~ω − 2γ1)

+γ1 log

[

2|εF |+ γ1γ1

]

δ(~ω − γ1)

, (103)

where εF is the Fermi energy and we assumed |εF | < γ1.We label the four bands in order of descending energyas 1, 2, 3, 4. The first term in equation (103) representsabsorption from band 2 to 3, the second from 2 to 4 orfrom 1 to 3, the third from 1 to 4, and the fourth from 3to 4 or from 1 to 2. Figure 12 (a) shows some examples ofcalculated dynamical conductivity Reσxx(ω) with severalvalues of the Fermi energy [229]. The curve for εF = 0has essentially no prominent structure except for a step-like increase corresponding to transitions from 2 to 4.With an increase in εF , a delta-function peak appears at~ω = γ1, corresponding to allowed transitions 3 to 4.In a magnetic field, an optical excitation by perpen-

dicular incident light is only allowed between the Lan-dau levels with n and n ± 1 for arbitrary combinationsof µ = H, L and s = ±1, since the matrix element ofthe velocity operator vx vanishes otherwise. Figure 12(b) shows some plots of Reσxx(ω) in magnetic fields atεF = 0 and zero temperature [230]. Dotted lines pene-trating panels represent the transition energies betweenseveral specific Landau levels as a continuous functionof ~ωB. Every peak position behaves as a linear func-tion of B ∝ ~ω2

B in weak field but it switches over to√B-dependence as the corresponding energy moves out

of the parabolic band region. In small magnetic fields,the peak structure is smeared out into the zero-field curvemore easily in the bilayer than in the monolayer, because

21

0

5

10

15

20

Dynam

ical C

onductivity (

units o

f g

vg

se

2/2

πh)

0.00

0.20

0.40

0.60

0.80

1.00

1.20

EF/γ1

(a)

0 1 20

1

2

hω / γ1

(0L, 1L±)

(1L , 2L±)±

(2L , 3L±)±

(-1L, 0H±)

(0L, 1H±)

(0H , 1L±)

±

(1L , 2H±)

±

(1H , 2L±)

±

(0H , 1H±)

±

Re

σxx (

un

its o

f g

vg

se

2/h

)

0.2 (4.5T)

0.3 (10T)

0.4 (18T)

0.5 (28T)

hωB / γ

1 = 0.1

(B ~ 1.1T)

hω / γ1

(b)

FIG. 12. Interband part of the dynamical conductivity ofbilayer graphene plotted against the frequency ω, in (a) zeromagnetic field with different εF ’s [229] (b) several magneticfields with εF = 0 [230]. Dashed curves in (b) indicate thetransition energies between several Landau levels.

the Landau level spacing is narrower in bilayer due to thefinite band mass.

VI. ORBITAL MAGNETISM

Graphite and related materials exhibit a strong or-bital diamagnetism which overcomes the Pauli spin para-magnetism. Theoretically the diamagnetic susceptibil-ity was calculated for graphite [121, 231, 232], graphiteintercalation compounds [233–236], as well as few-layergraphenes [237, 238]. In particular, monolayer graphenehas a strong diamagnetic singularity at Dirac point,which is expressed as a Delta function in Fermi energyεF [121, 239–242]. In the bilayer, the singularity is re-laxed by the modification of the band structure causedby the interlayer coupling as we will see in the following

[234, 237].

When the spectrum is composed of discrete Landaulevels εn, the thermodynamical potential is generallywritten as

Ω = − 1

β

gvgs2πl2B

∑

n

ϕ(εn), (104)

where β = 1/kBT , ϕ(ε) = log[

1+e−β(ε−ζ)]

with ζ beingthe chemical potential. In weak magnetic field, using theEuler-Maclaurin formula, the summation in n in equa-tion (104) can be written as an integral in a continuousvariable x with a residual term proportional to B2. Themagnetization M and the magnetic susceptibility χ canbe calculated by

M = −(∂Ω

∂B

)

ζ, χ =

∂M

∂B

∣

∣

∣

B=0= −

(∂2Ω

∂B2

)

ζ

∣

∣

∣

B=0.(105)

For monolayer graphene, the susceptibility is [121, 239]

χ = −gvgse2v2

6πc2

∫ ∞

−∞

(

−∂f(ε)∂ε

)

dε. (106)

At zero temperature, it becomes a delta function in Fermienergy,

χ(εF ) = −gvgse2v2

6πc2δ(εF ). (107)

The delta-function susceptibility of monolayer grapheneis strongly distorted by the interlayer coupling γ1. Forthe Hamiltonian of the symmetric bilayer graphene, theorbital susceptibility is calculated as [234, 237]

χ(ε) = gvgse2v2

4πc2γ1θ(γ1 − |ε|)

(

log|ε|γ1

+1

3

)

. (108)

The susceptibility diverges logarithmically at εF = 0, be-comes slightly paramagnetic near |εF | = γ1, and vanishesfor |εF | > γ1 where the higher subband enters. The in-tegration of χ in equation (108) over the Fermi energybecomes −gvgse2v2/(3πc2) independent of γ1, which isexactly twice as large as that of the monolayer graphene,equation (107).

The susceptibility was also calculated in the presenceof interlayer asymmetry [243]. Figure 13 (a) and (b) showthe density of states and the susceptibility, respectively,for bilayer graphene with U = 0, 0.2, and 0.5. Thesusceptibility diverges in the paramagnetic direction atthe band edges where the density of states also diverges.This huge paramagnetism can be interpreted as the Pauliparamagnetism induced by the valley pseudo-spin split-ting and diverging density of states [244]. The suscep-tibility vanishes in the energy region where the highersubband enters.

22

-0.5

0

0.5

1

-1.5 -1 -0.5 0 0.5 1 1.5

0

2

4

6

8

(a) DOS

(b) Susceptibility

∆ / γ1

0.2

0.5

0

∆ / γ1

0.2

0.5

0

DO

S (

un

its o

f g

vg

sγ 1

/4πh

2v

2)

Su

sce

ptib

ility

(u

nits o

f −g

vg

se

2v

2/π

c2γ 1

)

Energy (units of γ1)

-1.5 -1 -0.5 0 0.5 1 1.5

Energy (units of γ1)

FIG. 13. (a) Density of states, and (b) susceptibility of bilayergraphenes with the asymmetry gap U/γ1 = 0, 0.2, and 0.5[243]. In (b), the upward direction represents negative (i.e.,diamagnetic) susceptibility.

VII. PHONONS AND STRAIN

A. The influence of strain on electrons in bilayer

graphene

Deformation of a graphene sheet couples to the elec-tronic system and modifies the low-energy Hamiltonian.In monolayer graphene, static changes in distance andangles of the atomic bonds can be described as effec-tive scalar or vector potentials in the Dirac Hamiltonian[7, 245]. Bilayer graphene has extra degrees of freedom indeformation associated with the presence of two layers.It was shown that a band gap can be opened by givingdifferent distortions to the two layers or by pulling thetwo layers apart in the perpendicular direction [246–248].Rather than produce a band gap, it has been predicted

that homogeneous lateral strain in bilayer graphene canproduce a change in topology of the band structure at lowenergy [249–251]. This deformation causes tight-bindingparameters γ0 and γ3 to become dependent on the hop-ping direction and produces an additional term in thelow-energy two-band Hamiltonian (38)

hs =

(

0 w

w∗ 0

)

, (109)

where parameter w = |w|eiξθ depends on the microscopic

details of the deformation; it is non-zero only when therole of skew interlayer coupling γ3 is taken into account[249]. It is estimated that 1% strain would give |w| ∼6meV [249]. Taken with the quadratic term h0 in theHamiltonian (38), the low-energy bands with energy E =±ε1 are given by

ε21 = |w|2 − |w| p2m

cos (2ϕ+ θ) +

(

p2

2m

)2

. (110)

This describes a Lifshitz transition at energy εL = |w|,below which there are two Dirac points in the vicinityof each Brillouin zone corner [249–251], centred at mo-

mentum p ≈√

2m |w| =√

|w| γ1/v and angles ϕ = −θ/2and ϕ = π−θ/2. In general, there should be an interplay

between terms hs, equation (109), and hw, equation (38),leading to the possibility of employing strain to annihi-late two Dirac points and, thus, change the low energytopology of the bands from four to two Dirac points [249].The presence of two Dirac points would cause zero-

energy Landau levels to be eightfold degenerate; an ex-perimental signature of this state is predicted to be thepersistence of filling factor ν = ±4 in the low-field quan-tum Hall effect [249]. This contrasts with the Lifshitztransition that would occur in the presence of parameterγ3 without strain when there are four Dirac points, sec-tion II E, giving a degeneracy of sixteen and ν = ±8 atlow fields. In both cases, Berry phase 2π is conserved:two Dirac cones with Berry phase π each [249] or fourDirac cones with three of π and one of −π [12, 94]. It hasalso been predicted that the presence of the Lifshitz tran-sition will be noticeable in the low-energy conductivity atzero magnetic field [163, 169], and the particular case oftwo Dirac points in the presence of strain has recentlybeen analysed, too [252]. Note that the effect of lateralstrain on the low-energy topology of the band structureis qualitatively similar to that of a gapless nematic phasewhich possibly arises as the result of electron-electroninteractions in bilayer graphene [253–256].

B. Phonons in bilayer graphene

Raman spectroscopy has been a valuable tool in prob-ing the behaviour of phonons in graphite [257] and it maybe used to determine the number of layers in multilayergraphene [258], differentiating between monolayer and bi-layer. For an in-depth review of Raman spectroscopyof graphene including bilayer graphene see, for exam-ple, Refs. [259, 260]. The phonon spectrum of monolayergraphene has been calculated using a tight-binding force-constant model with parameters fit to Raman data [261],and with density functional theory [262–265]. There arethree acoustic (A) and three optical (O) branches consist-ing of longitudinal (L) and transverse (T) in-plane modesas well as out-of-plane (Z) modes. At the zone centre (theΓ point), the TA and LA modes display linear dispersionω ∼ q but the ZA mode is quadratic ω ∼ q2. The ZO

23

mode is at ∼ 890 cm−1 [262, 264], and the LO and TOmodes are degenerate (at ∼ 1600 cm−1). At the K point,the ZA and ZO modes (∼ 540 cm−1) and the LA and LOmodes (∼ 1240 cm−1) are degenerate, with TA modesat ∼ 1000 cm−1 and TO at ∼ 1300 cm−1. For undopedgraphene, owing to strong electron-phonon coupling, thehighest optical modes at the Γ and K point (i.e. the LOmode at the Γ point and the TO mode at the K point)display Kohn anomalies [266–268] whereby the phonondispersion ω(q) has an almost linear slope as observed,for example, in inelastic x-ray measurements of graphite[263, 268]. As graphene is a unique system in which theelectron or hole concentration can be tuned by an ex-ternal gate voltage, it was realised [269, 270] that thechange in electron density would also influence the be-haviour of the optical phonons through electron-phononcoupling and, in particular, a logarithmic singularityin their dispersion was predicted [269] when the Fermienergy εF is half of the energy of the optical phonon|εF | = ~ω/2. Subsequently, such tuning of phonon fre-quency and bandwidth by adjusting the electronic den-sity was observed in monolayer graphene through Ramanspectroscopy [271, 272].

The behaviour of phonons in bilayer graphene has beenobserved experimentally through Raman spectroscopy[76, 77, 273–279] and infrared spectroscopy [280, 281],with particular focus on optical phonon anomalies andthe influence of gating. Generally, the phonon spectrumof bilayer graphene, which has been calculated using den-sity functional theory [282, 283] and force-constant mod-els [284, 285], is similar to that of monolayer. Near theΓ point there are additional low-frequency modes. Thereis a doubly-degenerate rigid shear mode at ∼ 30 cm−1

[284, 285] observed through Raman spectroscopy [278]and an optical mode at ∼ 90 cm−1 which arises fromrelative motion of the layers in the vertical direction(perpendicular to the layer plane), known as a layer-breathing mode [286] and observed through Raman spec-troscopy [279]. At the Γ point, interlayer coupling causesthe LO/TO modes to split into two doubly-degeneratebranches where the higher (lower) frequency branch cor-responds to symmetric ‘in-phase’ (antisymmetric ‘out-of-phase’) relative motion of atoms on the two layers (in thein-plane direction). Analogously to the monolayer, it waspredicted that these optical phonons would be affectedby electron-phonon coupling, with a logarithmic singu-larity in the dispersion of the symmetric modes when theFermi energy εF is equal to half of the optical phononfrequency [287], and hybridisation of the symmetric andantisymmetric modes in the presence of interlayer poten-tial asymmetry [288, 289]. Experimentally, this anoma-lous phonon dispersion has been observed through Ra-man spectroscopy [77, 273–276] including the evolutionof two distinct components in the RamanG band for non-zero interlayer asymmetry [274–276]. The Raman spec-trum has also been studied for bilayer graphene in thepresence of Landau levels in a magnetic field [287, 290].

C. Optical phonon anomaly

In the following, we describe the anomalous opticalphonon spectrum in bilayer graphene taking into accountelectron-phonon coupling [287, 288]. Theoretically, it wasshown that a continuum model works well in describ-ing long-wavelength acoustic phonons [245] and opticalphonons [291] in graphene, and this theory was extendedto bilayer graphene [287, 288]. An optical phonon on onegraphene layer is represented by the relative displacementof two sub-lattice atoms A and B as

u(r) =∑

q,µ

√

~

4NMω0(bq,µ + b†−q,µ)eµ(q)e

iq·r, (111)

where N is the number of unit cells, M is the mass of acarbon atom, ω0 is the phonon frequency at the Γ point,q = (qx, qy) is the wave vector, and bq,µ and b†q,µ arethe creation and destruction operators, respectively. Theindex µ represents the modes (t for transverse and l forlongitudinal), and corresponding unit vectors are definedby ~el = iq/|q| and ~et = iz× q/|q|.The Hamiltonian of optical phonons is written as

Hph =∑

q,µ

~ω0

(

b†q,µbq,µ +1

2

)

, (112)

and the interaction with an electron at the K+ point is

HKint = −

√2β~v

a2CC

[σxuy(r)− σyux(r)] , (113)

where the Pauli matrix σi works on the space of(φA1, φB1) for the phonon on layer 1, and (φA2, φB2) forlayer 2. The dimensionless parameter β is related to thedependence of the hopping integral on the interatomicdistance, and is defined by β = −d log γ0/d log aCC. Weusually expect β ∼ 2. The strength of the electron-phonon interaction is characterized by a dimensionlessparameter

λ =gvgs4

36√3

π

~

2Ma21

~ω0

(

β

2

)2

. (114)

For M = 1.993× 1023g and ~ω0 = 0.196eV (correspond-ing to 1583 cm−1), we have λ ≈ 3 × 10−3(β/2)2. Forthe K− point, the interaction Hamiltonian is obtainedby replacing σi with −σ∗

i .The Green’s function of an optical phonon is given by

a 2 × 2 matrix associated with phonons on layers 1 and2. This is written as

D(q, ω) =2~ω0

(~ω)2 − (~ω0)2 − 2~ω0Π(q, ω)

≈ 1

~ω − ~ω0 − Π(q, ω0), (115)

where Π(q, ω) is the phonon’s self-energy, and the near-equality in the second line stands because the self-energy

24

-1.5 -1.0 -0.5 0.0 0.5 1.0 1.5

Electron Density (units of gvgsγ 2/2πhv2)

0.0

0.5

1.0

Bro

ad

en

ing

(u

nits o

f λ

ω0)

-1

0

1

2

Fre

qu

en

cy S

hift

(un

its o

f λ

ω0)

1

(a)

(b)

asymmetric

symmetric

FIG. 14. (a) Frequency shift and (b) broadening of the Γ-point optical phonon in a bilayer graphene [288]. Solid anddashed lines denote the high- and low-frequency modes, re-spectively, and the thin dotted lines in the top panel showthe frequencies for symmetric and antisymmetric modes cal-culated without inclusion of their mixing.

is much smaller than ~ω0. Then, the eigenmodes aregiven by eigenvectors |u〉 of ReΠ(q, ω0), and the fre-quency shift and broadening are obtained as the real andimaginary part of 〈u|Π(q, ω0)|u〉.In symmetric bilayer graphene (i.e., no interlayer po-

tential difference), eigenmodes are always classified intosymmetric and antisymmetric modes in which the dis-placement of the top and bottom layers is given by (u,u)for the former, and (u,−u) for the latter. The symmet-ric mode causes interband transitions between the con-duction band and valence band, while the antisymmetricmode contributes to the transitions between two conduc-tion bands (or between two valence bands). The potentialdifference between two layers gives rise to hybridisationof symmetric and antisymmetric modes [287].Figure 14 (a) and (b) show the calculated frequency

shift and broadening, respectively, as a function of elec-tron density ns [288]. Here we take ~ω0 = γ1/2, and in-troduce a phenomenological broadening factor of 0.1~ω0.We assume that ns is changed by the gate voltage, andappropriately take account of the band deformation dueto the interlayer potential difference when ns 6= 0, withthe self-consistent screening effect included. The thindotted lines in the top panel in Figure 14 (a) indicatethe frequencies for symmetric and antisymmetric modescalculated without inclusion of their mixing. The lowerand higher branches exactly coincide with symmetric andasymmetric modes at ns = 0 where the mixing is absent.The dip at the symmetric mode occurs when ~ω0 = 2εF ,i.e., the interband transition excites a valence electronexactly to the Fermi surface. The coupling between sym-metric and antisymmetric modes arises when ns 6= 0, and

makes an anti-crossing at the intersection.

VIII. ELECTRONIC INTERACTIONS

Generally speaking, the low-energy behaviour of elec-trons in bilayer graphene is well described by the tight-binding model without the need to explicitly incorporateelectron-electron interaction effects. Coulomb screeningand collective excitations have been described in a num-ber of theoretical papers [152, 292–300] and the impor-tance of interaction effects in a bilayer under externalgating [293, 301–307] has been stressed. Interaction ef-fects should also be important in the presence of a mag-netic field or at very low carrier density, particularly inclean samples.Bilayer graphene has quadratic bands which touch at

low energy resulting in a non-vanishing density of stateand it has been predicted to be unstable to electron-electron interactions at half filling. Trigonal warpingtends to cut off infrared singularities and, thus, finitecoupling strength is generally required to realise corre-lated ground states; if trigonal warping is neglected, thenarbitrarily weak interactions are sufficient. Since bilayergraphene possesses pseudospin (i.e., which layer) and val-ley degrees of freedom, in addition to real electron spin, itis possible to imagine a number of different broken sym-metry states that could prevail depending on model de-tails and parameter values. Suggestions include a ferro-magnetic [308], layer antiferromagnetic [14, 87, 309–312],ferroelectric [311, 313] or a charge density wave state[314]; topologically non-trivial phases with bulk gaps andgapless edge excitations such as an anomalous quantumHall state [87, 311, 315, 316] or a quantum spin Hall state[87, 311] (also called a spin flux state [256]); or a gaplessnematic phase [253–256, 317].Insulating states contribute a term proportional to σz

in the two-band Hamiltonian (38) with its sign corre-sponding to the distribution of layer, valley and spindegrees of freedom, indicated in figure 15, as manifestin their spin- and valley-dependent Hall conductivities[14, 87, 311]. Note that the quantum spin Hall stateproduces a term equivalent to that of intrinsic spin-orbitcoupling, equation (46), which describes a topological in-sulator state [99, 110, 111]. By way of contrast, the gap-less nematic phase has a qualitatively similar effect onthe spectrum of bilayer graphene as lateral strain [249],described in section VII, producing an additional term inthe two-band Hamiltonian of the form of equation (109),with parameter w taking the role of an order parameter.Experiments on suspended bilayer graphene devices

have found evidence for correlated states at very lowdensity and zero magnetic field [318–324]. Conductiv-ity measurements of double-gate devices [318] observed anon-monotonic dependence of the resistance on electricfield cumulating in a non-divergent resistance at zero fieldwhile compressibility measurements of single-gate devices[319] found an incompressible region near the charge neu-

25

K+ K-

quantum valley Hall

(a)

K+ K-

quantum spin Hall

(c)

K+ K-

quantum anomalous Hall

(b)

K+ K-

layer antiferromagnet

(d)

σz ξσz

ξsσz sσz

FIG. 15. Schematic of the distribution of spin, valley andlayer degrees of freedom in candidates for spontaneous gappedstates in bilayer graphene [14, 87, 311]. They each contributea term proportional to σz in the two-band Hamiltonian (38),with its sign depending on the valley ξ = ±1 and spin s =±1 orientation. Arrows indicate spin orientation, located atvalley K+ (solid) or K− (dashed) and on different layers (topor bottom) of a state at the top of the valence band.

trality point. These measurements were interpreted asbeing consistent with either the anomalous quantum Hallstate, in which the separate layers of the device are valleypolarised, or the gapless nematic phase.Subsequently, conductivity measurements on single-

gate devices [320] observed a weak temperature depen-dence of the width of the conductivity minimum nearzero carrier density, suggesting a suppressed density ofstates as compared to that expected for a parabolic dis-persion, as well as particularly robust cyclotron gaps atfilling factor ν = ±4, observations attributed to the pres-ence of the nematic phase.However, other experiments [321–324] observed insu-

lating states indicating the formation of ordered phaseswith energy gaps of about 2meV. There was evidencefor the existence of edge states in one of these exper-iment [321], but not in the others [322–324], and thelatter observations including their response to perpen-dicular electric field [322, 323] and tilted magnetic field[324] were seen as being consistent with a layer antiferro-magnetic state, in which the separate layers of the deviceare spin polarised, figure 15(d). At present, there appearto be contradicting experimental and theoretical results,but it should be noted that renormalisation group stud-ies [255, 256, 325] have highlighted the sensitivity of thephase diagram of bilayer graphene to microscopic details.In the absence of interactions, the low-energy Landau

level spectrum of bilayer graphene [9] consists of a seriesof fourfold (spin and valley) degenerate levels with aneightfold-degenerate level at zero energy, as described insection II J. The resulting Hall conductivity consists ofa series of plateaus at conventional integer positions of4e2/h, but with a double-sized step of 8e2/h across zero

density [8]. Interaction effects are expected to lift thelevel degeneracy of quantum Hall ferromagnet states atinteger filling factors [326–331]. Indeed, an insulatingstate at filling factor ν = 0 and complete splitting ofthe eightfold-degenerate level at zero energy have beenobserved with quantum states at filling factors ν = 0, 1, 2and 3 in high-mobility suspended bilayer graphene at lowfields (with all states resolved at B = 3T) [161, 332] andin samples on silicon substrates at high fields, typicallyabove 20T [333, 334].

The fractional quantum Hall effect has been observedrecently in monolayer graphene, both in suspended sam-ples [335, 336] and graphene on boron nitride [337], andthere is evidence for it in bilayer graphene [338], too.Strongly-correlated states at fractional filling factors andthe prospect of tuning their properties has been the fo-cus of recent theoretical attention [339–343]. Clearly, thenature of the electronic properties of bilayer graphene inhigh-mobility samples is a complicated problem, and it islikely to be an area of further intense experimental andtheoretical investigation in the following years.

IX. SUMMARY

This review focused on the single-particle theoryof electrons in bilayer graphene, in the shape of thetight-binding model and the related low-energy effectiveHamiltonian. Bilayer graphene has two unique proper-ties: massive chiral quasiparticles in two parabolic bandswhich touch at zero energy, and the possibility to con-trol an infrared gap between these low-energy bands byapplying an external gate potential. These features havea dramatic impact on many physical properties of bi-layer graphene including some described here: opticaland transport properties, orbital magnetism, phononsand strain. A number of topics were not covered here ingreat detail or at all; we refer the reader to relevant de-tailed reviews of graphene including electronic transport[176, 177], electronic and photonic devices [344], scan-ning tunnelling microscopy [345], Raman spectroscopy[259, 260], magnetism [346], spintronics and pseudospin-tronics [347], Andreev reflection at the interface with asuperconductor and Klein tunnelling [348], growth andapplications [21], and the properties of graphene in gen-eral [7, 349]. Finally, although the central features of thesingle-particle theory are already established, the samecan not be said of the influence of electronic interactions,which is likely to remain a subject of intense research,both theoretical and experimental, in the near future atleast.

The authors gratefully acknowledge colleagues forfruitful collaboration in graphene research, in particularT. Ando and V. I. Fal’ko, and we acknowledge fundingby the JST-EPSRC Japan-UK Cooperative ProgrammeGrant EP/H025804/1.

26

[1] Novoselov K S, Geim A K, Morozov S V, Jiang D, ZhangY, Dubonos S V, Grigorieva I V and Firsov A A 2004Science 306 666

[2] Novoselov K S, Geim A K, Morozov S V, Jiang D, Kat-snelson M I, Grigorieva I V, Dubonos S V and Firsov AA 2005 Nature 438 197

[3] Zhang Y B, Tan Y W, Stormer H L and Kim P 2005Nature 438 201

[4] DiVincenzo D P and Mele E J 1984 Phys. Rev. B 29

1685[5] Semenoff G W 1984 Phys. Rev. Lett. 53 2449[6] Haldane F D M 1988 Phys. Rev. Lett. 61 2015[7] Castro Neto A H, Guinea F, Peres N M R, Novoselov

K S and Geim A K 2009 Rev. Mod. Phys. 81 109[8] Novoselov K S, McCann E, Morozov S V, Fal’ko V I,

Katsnelson M I, Zeitler U, Jiang D, Schedin F and GeimA K 2006 Nature Phys. 2 177

[9] McCann E and Fal’ko V I 2006 Phys. Rev. Lett. 96

086805[10] Guinea F, Castro Neto A H and Peres N M R 2006

Phys. Rev. B 73 245426[11] Koshino M and Ando T 2007 Phys. Rev. B 76 085425[12] Manes J L, Guinea F and Vozmediano M A H 2007

Phys. Rev. B 75 155424[13] Nakamura M and Hirasawa L 2008 Phys. Rev. B 77

045429[14] Min H, Borghi G, Polini M and MacDonald A H 2008

Phys. Rev. B 77 041407[15] Min H and MacDonald A H 2008 Phys. Rev. B 77

155416[16] Ohta T, Bostwick A, Seyller T, Horn K and Rotenberg

E 2006 Science 313 951[17] McCann E 2006 Phys. Rev. B 74 161403(R)[18] Min H, Sahu B R, Banerjee S K and MacDonald A H

2007 Phys. Rev. B 75 155115[19] Oostinga J B, Heersche H B, Liu X, Morpurgo A F and

Vandersypen L M K 2007 Nature Mater. 7 151[20] Castro E V, Novoselov K S, Morozov S V, Peres N M

R, Lopes dos Santos J M B, Nilsson J, Guinea F, GeimA K and Castro Neto A H 2007 Phys. Rev. Lett. 99

216802[21] Novoselov K S, Fal’ko V I, Colombo L, Gellert P R,

Schwab M G and Kim K 2012 Nature 490 192[22] Dean C R, Young A F, Meric I, Lee C, Wang L, Sorgen-

frei S, Watanabe K, Taniguchi T, Kim P, Shepard K Land Hone J 2010 Nature Nanotech. 5 722

[23] Ghosh S, Bao W, Nika D L, Subrina S, Pokatilov E P,Lau C N and Balandin A A 2010 Nature Mater. 9 555

[24] Balandin A A 2011 Nature Mater. 10 569[25] Neek-Amal M and Peeters F M 2010 Phys. Rev. B 81

235421[26] Zhang Y Y, Wang C M, Cheng Y and Xiang Y 2011

Carbon 49 4511[27] Nair R R, Blake P, Grigorenko A N, Novoselov K S,

Booth T J, Stauber T, Peres N M R and Geim A K2008 Science 320 1308

[28] Bunch J S, Verbridge S S, Alden J S, an der Zande AM, Parpia J M, Craighead H G and McEuen P L 2008Nano Lett. 8 2458

[29] Elias D C, Nair R R, Mohiuddin T M G, Morozov SV, Blake P, Halsall M P, Ferrari A C, Boukhvalov D

W, Katsnelson M I, Geim A K and Novoselov K S 2009Science 323 610

[30] Bae S, Kim H, Lee Y, Xu X, Park J-S, Zheng Y, Bal-akrishnan J, Lei T, Kim H R, Song Y I, Kim Y-J, KimK S, Ozyilmaz B, Ahn J-H, Hong B H and Iijima S 2010Nature Nanotech. 5 574

[31] Xia F, Farmer D B, Lin Y-M and Avouris P 2010 NanoLett. 10 715

[32] Wang C-R, Lu W-S, Hao L, Lee W-L, Lee T-K, LinF, Cheng I-C and Chen J-Z 2011 Phys. Rev. Lett. 107186602

[33] Yan H, Li X, Chandra B, Tulevski G, Wu Y, Freitag M,Zhu W, Avouris P and Xia F 2012 Nature Nanotech. 7330

[34] Yan J, Kim M-H, Elle J A, Sushkov A B, Jenkins G S,Milchberg H M, Fuhrer M S and Drew H D 2012 NatureNanotech. 7 472

[35] Sugawara K, Kanetani K, Sato T and Takahashi T 2011AIP Adv. 1 022103

[36] Kanetani K, Sugawara K, Sato T, Shimizu R, Iwaya K,Hitosugi T and Takahashia T 2012 Proc. Nat. Acad. Sci.109 19610

[37] Gong L, Young R J, Kinloch I A, Riaz I, Jalil R andNovoselov K S 2012 ACS Nano 6 2086

[38] Young R J, Kinloch I A, Gong L and Novoselov K S2012 Compos. Sci. Technol. 72 1459

[39] Goossens A M, Driessen S C M, Baart T A, WatanabeK, Taniguchi T and Vandersypen L M K 2012 Nanoletters 12 4656

[40] Liu Z, Suenaga K, Harris P J F and Iijima S 2009 Phys.Rev. Lett. 102, 015501

[41] Lopes dos Santos J M B, Peres N M R and Castro NetoA H 2007 Phys. Rev. Lett. 99 256802

[42] Berger C, Song Z, Li X, Wu X, Brown N, Naud C,Mayou D, Li T, Hass J, Marchenkov A N, Conrad EH, First P N and de Heer W A 2006 Science 312 1191

[43] Hass J, Varchon F, Millan-Otoya J E, Sprinkle M,Sharma N, de Heer W A, Berger C, First P N, MagaudL and Conrad E H 2008 Phys. Rev. Lett. 100 125504

[44] Mele E J 2010 Phys. Rev. B 81 161405[45] Li G, Luican A, Lopes dos Santos J M B, Castro Neto A

H, Reina A, Kong J and Andrei E Y 2010 Nature Phys.6 109

[46] Luican A, Li G, Reina A, Kong J, Nair R R, NovoselovK S, Geim A K and Andrei E Y 2011 Phys. Rev. Lett.106 126802

[47] Schmidt H, Ludtke T, Barthold P, McCann E, Fal’ko VI and Haug R J 2008 Appl. Phys. Lett. 93 172108

[48] Ni Z, Wang Y, Yu T, You Y and Shen Z 2008 Phys.Rev. B 77 235403

[49] Min H, Bistritzer R, Su J-J and MacDonald A H 2008Phys. Rev. B 78 121401

[50] Kharitonov M Y and Efetov K B 2008 Phys. Rev. B 78

241401[51] Schmidt H, Ludtke T, Barthold P and Haug R J 2010

Physica E 42 699[52] Ponomarenko L A, Geim A K, Zhukov A A, Jalil R,

Morozov S V, Novoselov K S, Grigorieva I V, Hill E H,Cheianov V V, Falko V I, Watanabe K, Taniguchi Tand Gorbachev R V 2011 Nature Phys. 7 958

[53] Saito R, Dresselhaus M S and Dresselhaus G 1998 Phys-

27

ical Properties of Carbon Nanotubes (London: ImperialCollege Press)

[54] Nilsson J, Castro Neto A H, Guinea F and Peres N MR 2008 Phys. Rev. B 78 045405

[55] Zhang L M, Li Z Q, Basov D N, Fogler M M, Hao Zand Martin M C 2008 Phys. Rev. B 78 235408

[56] Li Z Q, Henriksen E A, Jiang Z, Hao Z, Martin M C,Kim P, Stormer H L and Basov D N 2009 Phys. Rev.Lett. 102 037403

[57] Latil S and Henrard L 2006 Phys. Rev. Lett. 97 036803[58] Koshino M and McCann E 2010 Phys. Rev. B 81 115315[59] Ashcroft NW and Mermin N D 1976 Solid-State Physics

(Belmont: Brooks/Cole)[60] McCann E 2012 Graphene Nanoelectronics: Metrol-

ogy, Synthesis, Properties and Applications Raza H (ed)(Berlin: Springer-Verlag) 237-275

[61] Partoens B and Peeters F M 2006 Phys. Rev. B 74

075404[62] Mucha-Kruczynski M, Tsyplyatyev O, Grishin A, Mc-

Cann E, Falko V I, Bostwick A and Rotenberg E 2008Phys. Rev. B 77 195403

[63] Mucha-Kruczynski M, McCann E and Falko V I 2010Semicond. Sci. Technol. 25 033001

[64] Slonczewski J C and Weiss P R 1958 Phys. Rev. 109

272[65] McClure J W 1957 Phys. Rev. 108 612[66] McClure J W 1960 Phys. Rev. 119 606[67] Dresselhaus M S and Dresselhaus G 2002 Adv. Phys. 51

1[68] Aoki M and Amawashi H 2007 Solid State Commun.

142 123[69] McCann E, Abergel D S L and Fal’ko V I 2007 Solid

State Commun. 143 110[70] Guinea F, Castro Neto A H and Peres N M R 2007 Solid

State Commun. 143 116[71] McCann E, Abergel D S L and Fal’ko V I 2007 Eur.

Phys. J. Special Topics 148 15[72] Guinea F, Castro Neto A H and Peres N M R 2007 Eur.

Phys. J. Special Topics 148 117[73] Gava P, Lazzeri M, Saitta A M and Mauri F 2009 Phys.

Rev. B 79 165431[74] Boukhvalov D W and Katsnelson M I 2008 Phys. Rev.

B 78 085413[75] Mucha-Kruczynski M, Abergel D S L, McCann E and

Falko V I 2009 J. Phys.: Condens. Matter 21 344206[76] Malard L M, Nilsson J, Elias D C, Brant J C, Plentz

F, Alves E S, Castro Neto A H and Pimenta M A 2007Phys. Rev. B 76 201401(R)

[77] Das A, Chakraborty B, Piscanec S, Pisana S, Sood A Kand Ferrari A C 2009 Phys. Rev. B 79 155417

[78] Henriksen E A, Jiang Z, Tung L-C, Schwartz M E,Takita M, Wang Y-J, Kim P and Stormer H L 2008Phys. Rev. Lett. 100 087403

[79] Kuzmenko A B, van Heumen E, van der Marel D, LerchP, Blake P, Novoselov K S and Geim A K 2009 Phys.Rev. B 79 115441

[80] Kuzmenko A B, Crassee I, van der Marel D, Blake Pand Novoselov K S 2009 Phys. Rev. B 80 165406

[81] Mak K F, Sfeir M Y, Misewich J A and Heinz T F 2010Proc. Nat. Acad. Sci. 107 14999

[82] Taychatanapat T, Watanabe K, Taniguchi T andJarillo-Herrero P 2011 Nature Phys. 7 621

[83] Trickey S B, Muller-Plathe F, Diercksen G H F andBoettger J C 1992 Phys. Rev. B 45 4460

[84] Koshino M and McCann E 2009 Phys. Rev. B 80 165409[85] Zhang F, Sahu S, Min H and MacDonald A H 2010

Phys. Rev. B 82 035409[86] Berry M V 1984 Proc. R. Soc. Lond. A 392 45[87] Zhang F, Jung J, Fiete G A, Niu Q and MacDonald A

H 2011 Phys. Rev. Lett. 106 156801[88] Ando T, Nakanishi T and Saito R 1998 J. Phys. Soc.

Jpn. 67 2857[89] Dresselhaus G 1974 Phys. Rev. B 10 3602[90] Nakao K 1976 J. Phys. Soc. Japan 40 761[91] Inoue M 1962 J. Phys. Soc. Japan 17 808[92] Gupta O P and Wallace P R 1972 Phys. Status. Solidi.

B 54 53[93] Lifshitz L M 1960 Zh. Exp. Teor. Fiz. 38 1565 [Sov.

Phys. JETP 11 1130][94] Mikitik G P and Sharlai Y 2008 Phys. Rev. B 77 113407[95] Wallace P R 1947 Phys. Rev. 71 622[96] Johnson J G and Dresselhaus G 1973 Phys. Rev. B 7

2275[97] Sasaki K, Murakami S and Saito R 2006 Appl. Phys.

Lett. 88 113110[98] Peres N M R, Guinea F and Castro Neto A H 2006

Phys. Rev. B 73 125411[99] Kane C L and Mele E J 2005 Phys. Rev. Lett. 95 226801

[100] Min H, Hill J E, Sinitsyn N A, Sahu B R, Kleinman Land MacDonald A H 2006 Phys. Rev. B 74 165310

[101] Huertas-Hernando D, Guinea F and Brataas A 2006Phys. Rev. B 74 155426

[102] Yao Y, Ye F, Qi X-L, Zhang S-C and Fang Z 2007 Phys.Rev. B 75 041401(R)

[103] Boettger J C and Trickey S B 2007 Phys. Rev. B 75

121402(R)[104] Gmitra M, Konschuh S, Ertler C, Ambrosch-Draxl C

and Fabian J 2009 Phys. Rev. B 80 235431[105] van Gelderen R and Morais Smith C 2010 Phys. Rev. B

81 125435[106] Guinea F 2010 New J. Phys. 12 083063[107] Liu H-W, Xie X C and Sun Q-F 2010 arXiv:1004.0881[108] McCann E and Koshino M 2010 Phys. Rev. B 81

241409(R)[109] Konschuh S, Gmitra M, Kochan D and Fabian J 2012

Phys. Rev. B 85 115423[110] Cortijo A, Grushin A G and Vozmediano M A H 2010

Phys. Rev. B 82 195438[111] Prada E, San-Jose P, Brey L and Fertig H A 2011 Solid

State Comm. 151 1075[112] Bychkov Y A and Rashba E I 1984 J. Phys. C 17 6039[113] Rashba E I 2009 Phys. Rev. B 79 161409[114] Rakyta P, Kormanyos A and Cserti J 2010 Phys. Rev.

B 82 113405[115] Qiao Z, Tse W-K, Jiang H, Yao Y and Niu Q 2011 Phys.

Rev. Lett. 107 256801[116] Mireles F and Schliemann J 2012 New J. Phys. 14

093026[117] Landau L D 1930 Z. Phys. 64 629[118] von Klitzing K, Dorda G and Pepper M 1980 Phys. Rev.

Lett. 45 494[119] Prange R E and Girvin S M (eds.) 1986 The Quantum

Hall Effect (New York: Springer-Verlag)[120] MacDonald A H (ed.) 1989 Quantum Hall Effect: A

Perspective (Boston: Kluwer)[121] McClure J W 1956 Phys. Rev. 104 666[122] Zheng Y and Ando T 2002 Phys. Rev. B 65 245420[123] Gusynin V P and Sharapov S G 2005 Phys. Rev. Lett.

28

95 146801[124] Herbut I F 2007 Phys. Rev. B 75 165411[125] Milton Pereira Jr. J, Peeters F M and Vasilopoulos P

2007 Phys. Rev. B 76 115419[126] Mucha-Kruczynski M, McCann E and Fal’ko V I 2009

Solid State Comm. 149 1111[127] Nakamura M, Castro E V and Dora B 2009 Phys. Rev.

Lett. 103 266804[128] Zhang L M, Fogler M M and Arovas D P 2011 Phys.

Rev. B 84 075451[129] Mak K F, Lui C H, Shan J and Heinz T F 2009 Phys.

Rev. Lett. 102 256405[130] Zhang Y, Tang T-T, Girit C, Hao Z, Martin M C, Zettl

A, Crommie M F, Shen Y R and Wang F 2009 Nature459 820

[131] Henriksen E A and Eisenstein J P 2010 Phys. Rev. B82 041412

[132] Young A F, Dean C R, Meric I, Sorgenfrei S, Ren H,Watanabe K, Taniguchi T, Hone J, Shepard K L and PKim 2012 Phys. Rev. B 85 235458

[133] Deshpande A, Bao W, Zhao Z, Lau C N and LeRoy BJ 2009 Appl. Phys. Lett. 95 243502

[134] Szafranek B N, Schall D, Otto M, Neumaier D and KurzH 2010 Appl. Phys. Lett. 96 112103

[135] Zou K and Zhu J 2010 Phys. Rev. B 82 081407(R)[136] Miyazaki H, Tsukagoshi K, Kanda A, Otani M and

Okada S 2010 Nano Lett. 10 3888[137] Jing L, Velasco Jr. J, Kratz P, Liu G, Bao W Z, Bock-

rath M and Lau C N 2010 Nano Lett. 10 4000[138] Taychatanapat T and Jarillo-Herrero P 2010 Phys. Rev.

Lett. 105 166601[139] Yan J and Fuhrer M S 2010 Nano Lett. 10 4521[140] Li J, Martin I, Buttiker M and Morpurgo A F 2011

Nature Phys. 7 38[141] Castro E V, Lopez-Sancho M P and Vozmediano M A

H 2010 Phys. Rev. Lett. 104 036802[142] Rossi E and Das Sarma S 2011 Phys. Rev. Lett. 107

155502[143] Abergel D S L, Min H K, Hwang E H and Das Sarma

S 2012 Phys. Rev. B 85 045411[144] Trushin M 2012 EPL 98 47007[145] Fogler M M and McCann E 2010 Phys. Rev. B 82

197401[146] Castro E V, Novoselov K S, Morozov S V, Peres N M R,

Lopes dos Santos J M B, Nilsson J, Guinea F, Geim AK and Castro Neto A H 2010 J. Phys.: Condens. Matter22 175503

[147] Koshino M and McCann E 2009 Phys. Rev. B 79 125443[148] Falkovsky L A 2009 Phys. Rev. B 80 113413[149] Nilsson J and Castro Neto A H 2007 Phys. Rev. Lett.

98 126801[150] Castro E V, Peres N M R and Lopes dos Santos J M B

2007 Phys. Stat. Sol. B 244 2311[151] Mkhitaryan V V and Raikh M E 2008 Phys. Rev. B 78

195409[152] Abergel D S L, Hwang E H and Das Sarma S 2011 Phys.

Rev. B 83 085429[153] Min H, Abergel D S L, Hwang E H and Das Sarma S

2011 Phys. Rev. B 84 041406(R)[154] Abergel D S L, Min H, Hwang E H and Das Sarma S

2011 Phys. Rev. B 84 195423[155] Rutter G M, Jung S, Klimov N N, Newell D B, Zhitenev

N B and Stroscio J A 2011 Nature Phys. 7 649[156] Avetisyan A A, Partoens B and Peeters F M 2009 Phys.

Rev. B 79 035421[157] Avetisyan A A, Partoens B and Peeters F M 2009 Phys.

Rev. B 80 195401[158] Koshino M 2010 Phys. Rev. B 81 125304[159] Gorbachev R V, Tikhonenko F V, Mayorov A S, Horsell

D W and Savchenko A K 2007 Phys. Rev. Lett. 98

176805[160] Morozov S V, Novoselov K S, Katsnelson M I, Schedin

F, Elias D C, Jaszczak J A and Geim A K 2008 Phys.Rev. Lett. 100 016602

[161] Feldman B E, Martin J and Yacoby A 2009 Nature Phys.5 889

[162] Xiao S, Chen J-H, Adam S, Williams E D and FuhrerM S 2010 Phys. Rev. B 82 041406

[163] Koshino M and Ando T 2006 Phys. Rev. B 73 245403[164] Nilsson J, Castro Neto A H, Guinea F and Peres N M

R 2006 Phys. Rev. Lett. 97 266801[165] Katsnelson M I 2006 Eur. Phys. J. B 52 151[166] Katsnelson M I 2007 Phys. Rev. B 76 073411[167] Cserti J 2007 Phys. Rev. B 75 033405[168] Snyman I and Beenakker C W J 2007 Phys. Rev. B 75

045322[169] Cserti J, Csordas A and David G 2007 Phys. Rev. Lett.

99 066802[170] Kechedzhi K, Fal’ko V I, McCann E and Altshuler B L

2007 Phys. Rev. Lett. 98 176806[171] Adam S and Das Sarma S 2008 Phys. Rev. B 77 115436[172] Das Sarma S, Hwang E H and Rossi E 2010 Phys. Rev.

B 81 161407(R)[173] Trushin M, Kailasvuori J, Schliemann J and MacDonald

A H 2010 Phys. Rev. B 82 155308[174] Hwang E H and Das Sarma S 2010 Phys. Rev. B 82

081409[175] Ferreira A, Viana-Gomes J, Nilsson J, Mucciolo E R,

Peres N M R and Castro Neto A H 2011 Phys. Rev. B83 165402

[176] Peres N M R 2010 Rev. Mod. Phys. 82 2673[177] Das Sarma S, Adam S, Hwang E H and Rossi E 2011

Rev. Mod. Phys. 83 407[178] Katsnelson M I, Novoselov K S and Geim A K 2006

Nature Phys. 2 620[179] Poole C J 2010 Solid State Commun. 150 632[180] Cheianov V V and Falko V I 2006 Phys. Rev. B 74

041403(R) 2006[181] Nilsson J, Castro Neto A H, Guinea F and Peres N M

R 2007 Phys. Rev. B 76 165416[182] Nakanishi T, Koshino M and Ando T 2010 Phys. Rev.

B 82 125428[183] Koshino M, Nakanishi T and Ando T 2010 Phys. Rev.

B 82 205436[184] Gonzalez J W, Santos H, Prada E, Brey L and Chico L

2011 Phys. Rev. B 83 205402[185] Barbier M, Vasilopoulos P, Peeters F M and Milton

Pereira Jr J 2009 Phys. Rev. B 79 155402[186] Ramezani Masir M, Vasilopoulos P and Peeters F M

2009 Phys. Rev. B 79 035409[187] Agrawal (Garg) N, Grover S, Ghosh S and Sharma M

2012 J. Phys.: Condens. Matter 24 175003[188] Fiori G and Iannaccone G 2009 IEEE Electr. Device L.

30 261[189] Martin I, Blanter Ya M and Morpurgo A F 2008 Phys.

Rev. Lett. 100 036804[190] Killi M, Wei T-C, Affleck I and Paramekanti A 2010

Phys. Rev. Lett. 104 216406

29

[191] Qiao Z, Jung J, Niu Q and MacDonald A H 2011 NanoLett. 11 3453

[192] Zarenia M, Pereira Jr. J M, Farias G A and Peeters FM 2011 Phys. Rev. B 84 125451

[193] San-Jose P, Prada E, McCann E and Schomerus H 2009Phys. Rev. Lett. 102 247204

[194] Li X G, Zhang Z Y and Xiao D 2010 Phys. Rev. B 81

195402[195] Xavier L J P, Pereira J M, Chaves A, Farias G A and

Peeters F M 2010 Appl. Phys. Lett. 96 212108[196] Schomerus H 2010 Phys. Rev. B 82 165409[197] Schomerus H 2007 Phys. Rev. B 76 045433[198] Tworzydlo J, Trauzettel B, Titov M, Rycerz A and

Beenakker C W J 2006 Phys. Rev. Lett. 96 246802[199] Landauer R 1970 Phil. Mag. 21 863[200] Buttiker M 1988 IBM J. Res. Dev. 32 317[201] Shon N H and Ando T 1998 J. Phys. Soc. Jpn. 67 2421[202] Koshino M 2009 New J. Phys. 11 095010[203] Ando T 2011 J. Phys. Soc. Jpn. 80 014707[204] Noro M, Koshino M and Ando T 2010 J. Phys. Soc.

Jpn. 79 094713[205] Altshuler B L, Khmelnitski D, Larkin A I and Lee P A

1980 Phys. Rev. B 22 5142[206] Hikami S, Larkin A I and Nagaoka Y 1980 Prog. Theor

Phys. 63 707[207] McEuen P L, Bockrath M, Cobden D H, Yoon Y-G and

Louie S G 1999 Phys. Rev. Lett. 83 5098[208] Suzuura H and Ando T 2002 Phys. Rev. Lett. 89 266603[209] Morozov S V, Novoselov K S, Katsnelson M I, Schedin

F, Ponomarenko L A, Jiang D and Geim A K 2006 Phys.Rev. Lett. 97 016801

[210] Morpurgo A F and Guinea F 2006 Phys. Rev. Lett. 97196804

[211] McCann E, Kechedzhi K, Fal’ko V I, Suzuura H, AndoT and Altshuler B L 2006 Phys. Rev. Lett. 97 146805

[212] Kechedzhi K, McCann E, Fal’ko V I, Suzuura H, AndoT and Altshuler B L 2007 Eur. Phys. J. Special Topics148 39

[213] Falko V I, Kechedzhi K, McCann E, Altshuler B L,Suzuura H and Ando T 2007 Solid State Comm. 14333

[214] Heersche H B, Jarillo-Herrero P, Oostinga J B, Vander-sypen L M K and Morpurgo A F 2007 Nature 446 56

[215] Wu X, Li X, Song Z, Berger C and de Heer W A 2007Phys. Rev. Lett. 98 136801

[216] Tikhonenko F V, Horsell D W, Gorbachev R V andSavchenko A K 2008 Phys. Rev. Lett. 100 056802

[217] Ki D-K, Jeong D, Choi J-H, Lee H-J and Park K-S 2008Phys. Rev. B 78 125409

[218] Tikhonenko F V, Kozikov A A, Savchenko A K andGorbachev R V 2009 Phys. Rev. Lett. 103 226801

[219] Lara-Avila S, Tzalenchuk A, Kubatkin S, Yakimova R,Janssen T J B M, Cedergren K, Bergsten T and FalkoV 2011 Phys. Rev. Lett. 107 166602

[220] McCann E 2009 Physics 2 98[221] Imura K-I, Kuramoto Y and Nomura K 2009 Phys. Rev.

B 80 085119[222] Imura K-I, Kuramoto Y and Nomura K 2010 Euro.

Phys. Lett. 89 17009[223] McCann E and Fal’ko V I 2012 Phys. Rev. Lett. 108

166606[224] Kechedzhi K, Fal’ko V I, McCann E and Altshuler B L

2007 Phys. Rev. Lett. 98 176806[225] Koshino M 2008 Phys. Rev. B 78, 155411

[226] Abergel D S L and Falko V I 2007 Phys. Rev. B 75

155430[227] Nicol E J and Carbotte J P 2008 Phys. Rev. B 77

155409[228] Koshino M and Ando T 2009 Solid State Commun. 149

1123[229] Ando T and Koshino M 2009 J. Phys. Soc. Jpn. 78

104716[230] Koshino M and Ando T 2008 Phys. Rev. B 77 115313[231] McClure J W 1960 Phys. Rev. 119 606[232] Sharma M P, Johnson L G and McClure J W 1974 Phys.

Rev. B 9 2467[233] Safran S A and DiSalvo F J 1979 Phys. Rev. B 20 4889[234] Safran S A 1984 Phys. Rev. B 30 421[235] Blinowski J and Rigaux C 1984 J. Phys. (Paris) 45 545[236] Saito R and Kamimura H 1986 Phys. Rev. B 33 7218[237] Koshino M and Ando T 2007 Phys. Rev. B 76 085425[238] Nakamura M and Hirasawa L 2008 Phys. Rev. B 77

045429[239] Koshino M and Ando T 2007 Phys. Rev. B 75 235333[240] Fukuyama H 2007 J. Phys. Soc. Jpn. 76 043711[241] Nakamura M 2007 Phys. Rev. B 76 113301[242] Ghosal A, Goswami P and Chakravarty S 2007 Phys.

Rev. B 75 115123[243] Koshino M and Ando T 2010 Phys. Rev. B 81 195431[244] Koshino M 2011 Phys. Rev. B 84 125427[245] Suzuura H and Ando T 2002 Phys. Rev. B 65 235412[246] Nanda B R K and Satpathy S 2009 Phys. Rev. B 80

165430[247] Choi S-M, Jhi S-H and Son Y-W 2010 Nano Lett. 10

3486[248] Verberck B, Partoens B, Peeters F M and Trauzettel B

2012 Phys. Rev. B 85 125403[249] Mucha-Kruczynski M, Aleiner I L and Falko V I 2011

Phys. Rev. B 84 041404[250] Son Y-W, Choi S-M, Hong Y P, Woo S and Jhi S-H

2011 Phys. Rev. B 84 155410[251] Mariani E, Pearce A J and von Oppen F 2012 Phys.

Rev. B 86 165448[252] Gradinar D A, Schomerus H and Fal’ko V I 2012 Phys.

Rev. B 85 165429[253] Vafek O and Yang K 2010 Phys. Rev. B 81 041401(R)[254] Lemonik Y, Aleiner I L, Toke C and Falko V I 2010

Phys. Rev. B 82 201408(R)[255] Throckmorton R E and Vafek O 2012 Phys. Rev. B 86

115447[256] Lemonik Y, Aleiner I L and Fal’ko V I 2012 Phys. Rev.

B 85 245451[257] Reich S and Thomsen C 2004 Phil. Trans. R. Soc. A

362 2271[258] Ferrari A C, Meyer J C, Scardaci V, Casiraghi C, Lazzeri

M, Mauri F, Piscanec S, Jiang D, Novoselov K S, RothS and Geim A K 2006 Phys. Rev. Lett. 97 187401

[259] Ferrari A C 2007 Solid State Commun. 143 47[260] Malard L M, Pimenta M A, Dresselhaus G and Dressel-

haus M S 2009 Phys. Rep. 473 51[261] Gruneis A, Saito R, Kimura T, Cancado L G, Pimenta

M A, Jorio A, Souza Filho A G, Dresselhaus G andDresselhaus M S 2002 Phys. Rev. B 65 155405

[262] Dubay O and Kresse G 2003 Phys. Rev. B 67 035401[263] Maultzsch J, Reich S, Thomsen C, Requardt H and Or-

dejon P 2004 Phys. Rev. Lett. 92 075501[264] Wirtz L and Rubio A 2004 Solid State Commun. 131

141

30

[265] Mounet N and Marzari N 2005 Phys. Rev. B 71 205214[266] Kohn W 1959 Phys. Rev. Lett. 2 393[267] Piscanec S, Lazzeri M, Mauri F, Ferrari A C and

Robertson J 2004 Phys. Rev. Lett. 93 185503[268] Lazzeri M, Piscanec S, Mauri F, Ferrari A C and

Robertson J 2006 Phys. Rev. B 73 155426[269] Ando T 2006 J. Phys. Soc. Jpn. 75 124701[270] Castro Neto A H and Guinea F 2007 Phys. Rev. B 75

045404[271] Pisana S, Lazzeri M, Casiraghi C, Novoselov K S, Geim

A K, Ferrari A C and Mauri F 2007 Nature Mater. 6198

[272] Yan J, Zhang Y, Kim P and Pinczuk A 2007 Phys. Rev.Lett. 98 166802

[273] Yan J, Henriksen E A, Kim P and Pinczuk A 2008 Phys.Rev. Lett. 101, 136804

[274] Malard L M, Elias D C, Alves E S and Pimenta M A2008 Phys. Rev. Lett. 101 257401

[275] Yan J, Villarson T, Henriksen E A, Kim P and PinczukA 2009 Phys. Rev. B 80 241417

[276] Bruna M and Borini S 2010 Phys. Rev. B 81 125421[277] Garcia J M, He R, Jiang M P, Yan J, Pinczuk A, Zuev Y

M, Kim K S, Kim P, Baldwin K, West K W and PfeifferL N 2010 Solid State Commun. 150 809

[278] Tan P H, Han W P, Zhao W J, Wu Z H, Chang K, WangH, Wang Y F, Bonini N, Marzari N, Pugno N, SaviniG, Lombardo A and Ferrari A C 2012 Nature Mater. 11294

[279] Lui C H, Malard L M, Kim S, Lantz G, Laverge F E,Saito R and Heinz T F 2012 Nano Lett. 12 5539

[280] Kuzmenko A B, Benfatto L, Cappelluti E, Crassee I,van der Marel D, Blake P, Novoselov K S and Geim AK 2009 Phys. Rev. Lett. 103 116804

[281] Tang T-T, Zhang Y, Park C-H, Geng B, Girit C, Hao Z,Martin M C, Zettl A, Crommie M F, Louie S G, ShenY R and Wang F 2010 Nature Nano. 5 32

[282] Yan J-A, Ruan W Y and Chou M Y 2008 Phys. Rev. B77 125401

[283] Saha S K, Waghmare U V, Krishnamurthy H R andSood A K 2008 Phys. Rev. B 78 165421

[284] Jiang J-W, Tang H, Wang B-S and Su Z-B 2008 Phys.Rev. B 77 235421

[285] Michel K H and Verberck B 2008 Phys. Rev. B 78

085424[286] Kitipornchai S, He X Q and Liew K M 2005 Phys. Rev.

B 72 075443[287] Ando T 2007 J. Phys. Soc. Jpn. 76 104711[288] Ando T and Koshino M 2009 J. Phys. Soc. Jpn. 78

034709[289] Gava P, Lazzeri M, Saitta A M and Mauri F 2009 Phys.

Rev. B 80 155422[290] Mucha-Kruczynski M, Kashuba O and Fal’ko V I 2010

Phys. Rev. B 82 045405[291] Ishikawa K and Ando T 2006 J. Phys. Soc. Jpn. 75

084713[292] Wang X F and Chakraborty T 2007 Phys. Rev. B 75

041404(R)[293] Stauber T, Peres N M R, Guinea F and Castro Neto A

H 2007 Phys. Rev. B 75 115425[294] Kusminskiy S V, Nilsson J, Campbell D K and Castro

Neto A H 2008 Phys. Rev. Lett. 100 106805[295] Hwang E H and Das Sarma S 2008 Phys. Rev. Lett. 101

156802[296] Kusminskiy S V, Campbell D K and Castro Neto A H

2009 EPL 85 58005[297] Borghi G, Polini M, Asgari R and MacDonald A H 2009

Phys. Rev. B 80 241402[298] Borghi G, Polini M, Asgari R and MacDonald A H 2010

Phys. Rev. B 82 155403[299] Sensarma R, Hwang E H and Das Sarma S 2010 Phys.

Rev. B 82 195428[300] Gamayun O V 2011 Phys. Rev. B 84 085112[301] Castro E V, Peres N M R, Stauber T and Silva N A P

2008 Phys. Rev. Lett. 100 186803[302] Dillenschneider R and Han J H 2008 Phys. Rev. B 78

045401[303] Sahu B, Min H, MacDonald A H and Banerjee S K 2008

Phys. Rev. B 78 045404[304] Park C-H and Louie S G 2010 Nano Lett. 10 426[305] Wang X-F and Chakraborty T 2010 Phys. Rev. B 81

081402[306] Cortijo A, Oroszlany L and Schomerus H 2010 Phys.

Rev. B 81 235422[307] Toke C and Fal’ko V I 2011 Phys. Rev. B 83 115455[308] Nilsson J, Castro Neto A H, Peres N M R and Guinea

F 2006 Phys. Rev. B 73 214418[309] Vafek O 2010 Phys. Rev. B 82 205106[310] Zhang F, Min H, Polini M and MacDonald A H 2010

Phys. Rev. B 81 041402(R)[311] Jung J, Zhang F and MacDonald A H 2011 Phys. Rev.

B 83 115408[312] Kharitonov M 2012 Phys. Rev. B 86 195435[313] Nandkishore R and Levitov L 2010 Phys. Rev. Lett. 104

156803[314] Dahal H P, Wehling T O, Bedell K S, Zhu J-X and

Balatsky A V 2010 Physica B 405 2241[315] Nandkishore R and Levitov L arXiv:1002.1966 (unpub-

lished).[316] Nandkishore R and Levitov L 2010 Phys. Rev. B 82

115124[317] Sun K, Yao H, Fradkin E and Kivelson S A 2009 Phys.

Rev. Lett. 103 046811[318] Weitz R T, Allen M T, Feldman B E, Martin J and

Yacoby A 2010 Science 330 812[319] Martin J, Feldman B E, Weitz R T, Allen M T and

Yacoby A 2010 Phys. Rev. Lett. 105 256806[320] Mayorov A S, Elias D C, Mucha-Kruczynski M, Gor-

bachev R V, Tudorovskiy T, Zhukov A, Morozov S V,Katsnelson M I, Falko V I, Geim A K and Novoselov KS 2011 Science 333 860

[321] Freitag F, Trbovic J, Weiss M and Schonenberger C2012 Phys. Rev. Lett. 108 076602

[322] Velasco Jr. J, Jing L, Bao W, Lee Y, Kratz P, Aji V,Bockrath M, Lau C N, Varma C, Stillwell R, SmirnovD, Zhang F, Jung J and MacDonald A H 2012 NatureNanotech. 7 156

[323] Bao W, Velasco Jr. J, Zhang F, Jing L, Standley B,Smirnov D, Bockrath M, MacDonald A H and Lau C N2012 Proc. Nat. Acad. Sci. 109 10802

[324] Veligura A, van Elferen H J, Tombros N, Maan J C,Zeitler U and van Wees B J 2012 Phys. Rev. B 85

155412[325] Zhang F, Min H and MacDonald A H 2012 Phys. Rev.

B 86 155128[326] Nomura K and MacDonald A H 2006 Phys. Rev. Lett.

96 256602[327] Barlas Y, Cote R, Nomura K and MacDonald A H 2008

Phys. Rev. Lett. 101 097601

31

[328] Shizuya K 2009 Phys. Rev. B 79 165402[329] Abanin D A, Parameswaran S A and Sondhi S L 2009

Phys. Rev. Lett. 103 076802[330] Gorbar E V, Gusynin V P and Miransky V A 2010 Phys.

Rev. B 81 155451[331] Gorbar E V, Gusynin V P, Jia J and Miransky V A

2011 Phys. Rev. B 84 235449[332] van Elferen H J, Veligura A, Kurganova E V, Zeitler U,

Maan J C, Tombros N, Vera-Marun I J and van WeesB J 2012 Phys. Rev. B 85 115408

[333] Zhao Y, Cadden-Zimansky P, Jiang Z and Kim P 2010Phys. Rev. Lett. 104 066801

[334] Kim S, Lee K and Tutuc E 2011 Phys. Rev. Lett. 107016803

[335] Du X, Shachko I, Duerr F, Luican A and Andrei E Y2009 Nature 462 192

[336] Bolotin K I, Ghahari F, Shulman M D, Stormer H Land Kim P 2009 Nature 462 196

[337] Dean C R, Young A F, Cadden-Zimansky P, Wang L,Ren H, Watanabe K, Taniguchi T, Kim P, Hone J andShepard K L 2011 Nature Phys. 7 693

[338] Bao W, Zhao Z, Zhang H, Liu G, Kratz P, Jing L, Ve-

lasco Jr J, Smirnov D and Lau C N 2010 Phys. Rev.Lett. 105 246601

[339] Shibata N and Nomura K 2009 J. Phys. Soc. Jpn. 78104708

[340] Apalkov V M and Chakraborty T 2010 Phys. Rev. Lett.105 036801

[341] Apalkov V M and Chakraborty T 2011 Phys. Rev. Lett.107 186803

[342] Papic Z, Abanin D A, Barlas Y and Bhatt R N 2011Phys. Rev. B 84 241306(R)

[343] Snizhko K, Cheianov V and Simon S H 2012 Phys. Rev.B 85 201415(R)

[344] Avouris P 2010 Nano Lett. 10 4285[345] Andrei E Y, Li G and Du X 2012 Rep. Prog. Phys. 75

056501[346] Yazyev O V 2010 Rep. Prog. Phys. 73 056501[347] Pesin D and MacDonald A H 2012 Nature Mat. 11 409[348] Beenakker C W J 2008 Rev. Mod. Phys. 80 1337[349] Abergel D S L, Apalkov V, Berashevich J, Ziegler K and

Chakraborty T 2010 Adv. Phys. 59 261

Recommended